# Supplementary Information (SI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2025

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_bep2o6
_database_code_depnum_ccdc_archive 'CCDC 2384141'
loop_
_audit_author_name
_audit_author_address
'Xia Zhang'
;Shanxi Normal University
China
;
_audit_update_record             
;
2024-09-14 deposited with the CCDC.	2025-04-25 downloaded from the CCDC.
;
_audit_creation_date             2024-09-12
_audit_creation_method           
;
Olex2 1.5
(compiled 2024.02.16 svn.r378c4104 for OlexSys, GUI svn.r6928)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        
;
 ?
;
_chemical_formula_moiety         'Be O6 P2'
_chemical_formula_sum            'Be O6 P2'
_chemical_formula_weight         166.95
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Be Be 0.0005 0.0002 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 1 21 1'
_space_group_name_Hall           'P 2yb'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   7.084(2)
_cell_length_b                   8.586(3)
_cell_length_c                   14.092(7)
_cell_angle_alpha                90
_cell_angle_beta                 94.06(3)
_cell_angle_gamma                90
_cell_volume                     855.0(6)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    3766
_cell_measurement_temperature    273.15
_cell_measurement_theta_max      56.88
_cell_measurement_theta_min      2.78
_shelx_estimated_absorpt_T_max   0.862
_shelx_estimated_absorpt_T_min   0.676
_exptl_absorpt_coefficient_mu    0.953
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.594
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             656
_exptl_crystal_size_max          0.445
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.16
_exptl_special_details           
;
 ?
;
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0260
_diffrn_reflns_av_unetI/netI     0.0446
_diffrn_reflns_Laue_measured_fraction_full 0.983
_diffrn_reflns_Laue_measured_fraction_max 0.775
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            6768
_diffrn_reflns_point_group_measured_fraction_full 0.964
_diffrn_reflns_point_group_measured_fraction_max 0.729
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.432
_diffrn_reflns_theta_min         2.780
_diffrn_ambient_temperature      273.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.983
_diffrn_measured_fraction_theta_max 0.775
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.773
_reflns_Friedel_fraction_full    0.943
_reflns_Friedel_fraction_max     0.676
_reflns_number_gt                3800
_reflns_number_total             4131
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         0.521
_refine_diff_density_min         -0.349
_refine_diff_density_rms         0.082
_refine_ls_abs_structure_details 
;
 Flack x determined using 1542 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   -0.01(5)
_refine_ls_extinction_coef       0.099(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     326
_refine_ls_number_reflns         4131
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0381
_refine_ls_R_factor_gt           0.0328
_refine_ls_restrained_S_all      1.036
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0386P)²+0.5175P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0793
_refine_ls_wR_factor_ref         0.0823
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
P1 P 0.61338(14) 0.30243(13) 0.32738(7) 0.0121(2) Uani 1 1 d . . . . .
P3 P 0.17446(14) 0.26671(12) 0.55526(7) 0.0130(2) Uani 1 1 d . . . . .
P5 P 0.60115(14) 0.29920(13) 0.82056(7) 0.0125(2) Uani 1 1 d . . . . .
P7 P 0.85011(14) 0.75144(13) 0.94185(7) 0.0125(2) Uani 1 1 d . . . . .
P8 P 0.44019(14) 0.77954(13) 0.97162(7) 0.0138(2) Uani 1 1 d . . . . .
P4 P 0.09883(14) 0.03757(13) 0.70721(7) 0.0126(3) Uani 1 1 d . . . . .
P6 P 0.91475(14) 0.51613(13) 0.79659(7) 0.0125(3) Uani 1 1 d . . . . .
P2 P 0.59021(14) 0.25315(15) 0.53530(7) 0.0180(3) Uani 1 1 d . . . . .
O9 O 0.0748(5) 0.4163(4) 0.5523(2) 0.0281(8) Uani 1 1 d . . . . .
O18 O 1.1095(4) 0.4960(4) 0.8334(2) 0.0191(7) Uani 1 1 d . . . . .
O16 O 0.8790(5) 0.5387(4) 0.6943(2) 0.0219(7) Uani 1 1 d . . . . .
O12 O 0.1738(4) 0.0506(4) 0.8053(2) 0.0196(6) Uani 1 1 d . . . . .
O24 O 0.3321(4) 0.9237(4) 0.9583(2) 0.0241(7) Uani 1 1 d . . . . .
O14 O 0.4640(4) 0.4207(4) 0.7956(3) 0.0266(8) Uani 1 1 d . . . . .
O23 O 0.3936(5) 0.6382(4) 0.9177(2) 0.0260(8) Uani 1 1 d . . . . .
O15 O 0.8056(4) 0.3692(4) 0.8346(3) 0.0278(8) Uani 1 1 d . . . . .
O21 O 0.6517(4) 0.8272(4) 0.9570(3) 0.0241(7) Uani 1 1 d . . . . .
O11 O -0.1002(5) -0.0017(5) 0.6919(3) 0.0291(8) Uani 1 1 d . . . . .
O3 O 0.7795(4) 0.4195(4) 0.3521(2) 0.0236(7) Uani 1 1 d . . . . .
O19 O 0.9764(5) 0.8781(4) 0.9187(3) 0.0285(8) Uani 1 1 d . . . . .
O13 O 0.6133(5) 0.1678(4) 0.7550(2) 0.0295(8) Uani 1 1 d . . . . .
O2 O 0.4417(5) 0.3834(4) 0.2970(3) 0.0321(9) Uani 1 1 d . . . . .
O17 O 0.8104(5) 0.6532(4) 0.8488(2) 0.0271(8) Uani 1 1 d . . . . .
O20 O 0.9049(5) 0.6509(4) 1.0224(2) 0.0254(7) Uani 1 1 d . . . . .
O10 O 0.1456(6) 0.1966(4) 0.6572(2) 0.0339(9) Uani 1 1 d . . . . .
O1 O 0.6872(5) 0.1850(4) 0.2623(3) 0.0325(9) Uani 1 1 d . . . . .
O22 O 0.5623(5) 0.2283(4) 0.9210(2) 0.0286(8) Uani 1 1 d . . . . .
O4 O 0.5850(5) 0.2215(5) 0.4256(2) 0.0315(9) Uani 1 1 d . . . . .
O8 O 0.1357(6) 0.1538(4) 0.4801(2) 0.0305(8) Uani 1 1 d . . . . .
O7 O 0.3884(5) 0.3113(5) 0.5579(3) 0.0356(9) Uani 1 1 d . . . . .
O5 O 0.7138(6) 0.3816(5) 0.5595(3) 0.0466(13) Uani 1 1 d . . . . .
O6 O 0.6220(6) 0.0983(5) 0.5784(2) 0.0372(10) Uani 1 1 d . . . . .
Be2 Be 0.6770(7) 0.0601(6) 0.1799(4) 0.0120(10) Uani 1 1 d . . . . .
Be1 Be 0.6779(7) 0.0388(7) 0.6830(4) 0.0155(10) Uani 1 1 d . . . . .
Be4 Be 0.1429(7) 1.0018(6) 0.9147(4) 0.0146(10) Uani 1 1 d . . . . .
Be3 Be -0.1171(7) 0.4990(7) 0.5820(4) 0.0155(11) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
P1 O3 1.568(3) . ?
P1 O2 1.440(3) . ?
P1 O1 1.483(4) . ?
P1 O4 1.575(3) . ?
P3 O9 1.465(4) . ?
P3 O10 1.584(4) . ?
P3 O8 1.448(3) . ?
P3 O7 1.561(3) . ?
P5 O14 1.452(4) . ?
P5 O15 1.568(3) . ?
P5 O13 1.465(4) . ?
P5 O22 1.582(3) . ?
P7 O21 1.577(3) . ?
P7 O19 1.460(3) . ?
P7 O17 1.567(3) . ?
P7 O20 1.457(3) . ?
P8 O24 1.461(4) . ?
P8 O23 1.457(4) . ?
P8 O21 1.581(3) . ?
P8 O22 1.578(3) 2_657 ?
P4 O12 1.449(3) . ?
P4 O11 1.451(3) . ?
P4 O3 1.603(3) 2_646 ?
P4 O10 1.583(4) . ?
P6 O18 1.450(3) . ?
P6 O16 1.458(3) . ?
P6 O15 1.592(3) . ?
P6 O17 1.597(3) . ?
P2 O4 1.567(3) . ?
P2 O7 1.568(3) . ?
P2 O5 1.434(4) . ?
P2 O6 1.472(4) . ?
O9 Be3 1.615(6) . ?
O18 Be2 1.633(6) 2_756 ?
O16 Be3 1.622(6) 1_655 ?
O12 Be4 1.627(6) 1_545 ?
O24 Be4 1.583(6) . ?
O14 Be2 1.612(6) 2_656 ?
O23 Be2 1.580(6) 2_656 ?
O11 Be1 1.606(6) 1_455 ?
O19 Be4 1.591(6) 1_655 ?
O13 Be1 1.592(6) . ?
O2 Be1 1.616(7) 2_656 ?
O20 Be4 1.606(6) 2_647 ?
O1 Be2 1.579(6) . ?
O8 Be3 1.592(7) 2_546 ?
O5 Be3 1.580(6) 1_655 ?
O6 Be1 1.584(6) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 P1 O4 103.21(18) . . ?
O2 P1 O3 111.2(2) . . ?
O2 P1 O1 118.2(2) . . ?
O2 P1 O4 108.5(2) . . ?
O1 P1 O3 106.3(2) . . ?
O1 P1 O4 108.5(2) . . ?
O9 P3 O10 105.4(2) . . ?
O9 P3 O7 104.5(2) . . ?
O8 P3 O9 120.0(2) . . ?
O8 P3 O10 112.3(2) . . ?
O8 P3 O7 108.4(2) . . ?
O7 P3 O10 105.0(2) . . ?
O14 P5 O15 110.6(2) . . ?
O14 P5 O13 118.0(2) . . ?
O14 P5 O22 109.7(2) . . ?
O15 P5 O22 104.59(19) . . ?
O13 P5 O15 106.3(2) . . ?
O13 P5 O22 106.8(2) . . ?
O19 P7 O21 106.8(2) . . ?
O19 P7 O17 106.9(2) . . ?
O17 P7 O21 103.08(18) . . ?
O20 P7 O21 109.3(2) . . ?
O20 P7 O19 118.8(2) . . ?
O20 P7 O17 110.8(2) . . ?
O24 P8 O21 104.9(2) . . ?
O24 P8 O22 108.58(19) . 2_657 ?
O23 P8 O24 122.8(2) . . ?
O23 P8 O21 109.3(2) . . ?
O23 P8 O22 104.5(2) . 2_657 ?
O22 P8 O21 105.82(19) 2_657 . ?
O12 P4 O11 116.5(2) . . ?
O12 P4 O3 111.81(19) . 2_646 ?
O12 P4 O10 106.5(2) . . ?
O11 P4 O3 109.1(2) . 2_646 ?
O11 P4 O10 111.5(2) . . ?
O10 P4 O3 100.2(2) . 2_646 ?
O18 P6 O16 117.66(19) . . ?
O18 P6 O15 104.93(19) . . ?
O18 P6 O17 112.48(19) . . ?
O16 P6 O15 112.6(2) . . ?
O16 P6 O17 107.7(2) . . ?
O15 P6 O17 100.2(2) . . ?
O4 P2 O7 107.3(2) . . ?
O5 P2 O4 109.8(2) . . ?
O5 P2 O7 104.9(2) . . ?
O5 P2 O6 121.6(3) . . ?
O6 P2 O4 104.0(2) . . ?
O6 P2 O7 108.6(2) . . ?
P3 O9 Be3 142.3(3) . . ?
P6 O18 Be2 141.7(3) . 2_756 ?
P6 O16 Be3 157.4(3) . 1_655 ?
P4 O12 Be4 145.0(3) . 1_545 ?
P8 O24 Be4 146.2(3) . . ?
P5 O14 Be2 153.6(3) . 2_656 ?
P8 O23 Be2 148.6(3) . 2_656 ?
P5 O15 P6 136.7(2) . . ?
P7 O21 P8 140.6(2) . . ?
P4 O11 Be1 153.7(4) . 1_455 ?
P1 O3 P4 135.4(2) . 2_656 ?
P7 O19 Be4 166.6(3) . 1_655 ?
P5 O13 Be1 166.1(4) . . ?
P1 O2 Be1 142.1(3) . 2_656 ?
P7 O17 P6 136.1(2) . . ?
P7 O20 Be4 147.9(3) . 2_647 ?
P4 O10 P3 140.9(2) . . ?
P1 O1 Be2 156.5(3) . . ?
P8 O22 P5 139.9(3) 2_647 . ?
P2 O4 P1 142.7(3) . . ?
P3 O8 Be3 164.8(3) . 2_546 ?
P3 O7 P2 144.5(3) . . ?
P2 O5 Be3 168.4(4) . 1_655 ?
P2 O6 Be1 134.1(4) . . ?
O14 Be2 O18 111.6(4) 2_646 2_746 ?
O23 Be2 O18 106.3(3) 2_646 2_746 ?
O23 Be2 O14 109.8(3) 2_646 2_646 ?
O1 Be2 O18 108.6(3) . 2_746 ?
O1 Be2 O14 110.1(4) . 2_646 ?
O1 Be2 O23 110.3(4) . 2_646 ?
O11 Be1 O2 109.3(4) 1_655 2_646 ?
O13 Be1 O11 115.2(4) . 1_655 ?
O13 Be1 O2 106.6(4) . 2_646 ?
O6 Be1 O11 108.7(4) . 1_655 ?
O6 Be1 O13 107.8(4) . . ?
O6 Be1 O2 109.2(4) . 2_646 ?
O24 Be4 O12 108.0(4) . 1_565 ?
O24 Be4 O19 108.2(4) . 1_455 ?
O24 Be4 O20 109.2(4) . 2_657 ?
O19 Be4 O12 110.8(4) 1_455 1_565 ?
O19 Be4 O20 109.1(4) 1_455 2_657 ?
O20 Be4 O12 111.4(4) 2_657 1_565 ?
O9 Be3 O16 114.7(4) . 1_455 ?
O8 Be3 O9 105.3(4) 2_556 . ?
O8 Be3 O16 110.7(4) 2_556 1_455 ?
O5 Be3 O9 107.9(4) 1_455 . ?
O5 Be3 O16 105.4(4) 1_455 1_455 ?
O5 Be3 O8 113.0(4) 1_455 2_556 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
P1 O1 Be2 O18 178.8(7) . . . 2_746 ?
P1 O1 Be2 O14 -58.8(10) . . . 2_646 ?
P1 O1 Be2 O23 62.6(10) . . . 2_646 ?
P3 O9 Be3 O16 76.2(6) . . . 1_455 ?
P3 O9 Be3 O8 -161.8(4) . . . 2_556 ?
P3 O9 Be3 O5 -40.9(7) . . . 1_455 ?
P5 O13 Be1 O11 26.4(16) . . . 1_655 ?
P5 O13 Be1 O2 147.8(13) . . . 2_646 ?
P5 O13 Be1 O6 -95.1(14) . . . . ?
P8 O24 Be4 O12 -87.7(6) . . . 1_565 ?
P8 O24 Be4 O19 32.4(7) . . . 1_455 ?
P8 O24 Be4 O20 151.0(5) . . . 2_657 ?
P2 O6 Be1 O11 -100.5(5) . . . 1_655 ?
P2 O6 Be1 O13 24.9(6) . . . . ?
P2 O6 Be1 O2 140.3(4) . . . 2_646 ?
O9 P3 O10 P4 137.4(4) . . . . ?
O9 P3 O8 Be3 -160.4(13) . . . 2_546 ?
O9 P3 O7 P2 -156.2(5) . . . . ?
O18 P6 O16 Be3 57.1(9) . . . 1_655 ?
O18 P6 O15 P5 -174.2(4) . . . . ?
O18 P6 O17 P7 -14.2(5) . . . . ?
O16 P6 O18 Be2 39.3(5) . . . 2_756 ?
O16 P6 O15 P5 -45.1(4) . . . . ?
O16 P6 O17 P7 -145.5(4) . . . . ?
O12 P4 O11 Be1 82.4(8) . . . 1_455 ?
O12 P4 O10 P3 156.2(4) . . . . ?
O24 P8 O23 Be2 38.0(7) . . . 2_656 ?
O24 P8 O21 P7 -167.1(4) . . . . ?
O14 P5 O15 P6 -26.7(4) . . . . ?
O14 P5 O13 Be1 120.7(14) . . . . ?
O14 P5 O22 P8 -62.6(4) . . . 2_647 ?
O23 P8 O24 Be4 14.5(7) . . . . ?
O23 P8 O21 P7 -33.8(4) . . . . ?
O15 P5 O14 Be2 -83.7(7) . . . 2_656 ?
O15 P5 O13 Be1 -4.1(15) . . . . ?
O15 P5 O22 P8 56.1(4) . . . 2_647 ?
O15 P6 O18 Be2 165.3(5) . . . 2_756 ?
O15 P6 O16 Be3 -65.1(8) . . . 1_655 ?
O15 P6 O17 P7 96.7(4) . . . . ?
O21 P7 O19 Be4 122.2(15) . . . 1_655 ?
O21 P7 O17 P6 -164.1(4) . . . . ?
O21 P7 O20 Be4 60.1(7) . . . 2_647 ?
O21 P8 O24 Be4 139.7(6) . . . . ?
O21 P8 O23 Be2 -85.2(6) . . . 2_656 ?
O11 P4 O12 Be4 21.3(6) . . . 1_545 ?
O11 P4 O10 P3 -75.7(5) . . . . ?
O3 P1 O2 Be1 -36.8(6) . . . 2_656 ?
O3 P1 O1 Be2 -151.3(8) . . . . ?
O3 P1 O4 P2 36.2(5) . . . . ?
O3 P4 O12 Be4 -105.2(5) 2_646 . . 1_545 ?
O3 P4 O11 Be1 -149.8(7) 2_646 . . 1_455 ?
O3 P4 O10 P3 39.7(5) 2_646 . . . ?
O19 P7 O21 P8 171.2(4) . . . . ?
O19 P7 O17 P6 83.6(4) . . . . ?
O19 P7 O20 Be4 -177.1(6) . . . 2_647 ?
O13 P5 O14 Be2 153.7(7) . . . 2_656 ?
O13 P5 O15 P6 102.5(4) . . . . ?
O13 P5 O22 P8 168.5(4) . . . 2_647 ?
O2 P1 O3 P4 -68.1(4) . . . 2_656 ?
O2 P1 O1 Be2 -25.6(10) . . . . ?
O2 P1 O4 P2 -81.8(5) . . . . ?
O17 P7 O21 P8 58.7(4) . . . . ?
O17 P7 O19 Be4 -128.0(15) . . . 1_655 ?
O17 P7 O20 Be4 -52.8(7) . . . 2_647 ?
O17 P6 O18 Be2 -86.8(5) . . . 2_756 ?
O17 P6 O16 Be3 -174.5(8) . . . 1_655 ?
O17 P6 O15 P5 69.1(4) . . . . ?
O20 P7 O21 P8 -59.1(4) . . . . ?
O20 P7 O19 Be4 -1.8(16) . . . 1_655 ?
O20 P7 O17 P6 -47.3(4) . . . . ?
O10 P3 O9 Be3 -41.3(6) . . . . ?
O10 P3 O8 Be3 -35.7(14) . . . 2_546 ?
O10 P3 O7 P2 93.1(5) . . . . ?
O10 P4 O12 Be4 146.3(5) . . . 1_545 ?
O10 P4 O11 Be1 -40.1(8) . . . 1_455 ?
O1 P1 O3 P4 61.8(4) . . . 2_656 ?
O1 P1 O2 Be1 -160.1(5) . . . 2_656 ?
O1 P1 O4 P2 148.6(4) . . . . ?
O22 P5 O14 Be2 31.2(8) . . . 2_656 ?
O22 P5 O15 P6 -144.7(4) . . . . ?
O22 P5 O13 Be1 -115.3(14) . . . . ?
O22 P8 O24 Be4 -107.5(6) 2_657 . . . ?
O22 P8 O23 Be2 161.9(6) 2_657 . . 2_656 ?
O22 P8 O21 P7 78.2(4) 2_657 . . . ?
O4 P1 O3 P4 175.8(3) . . . 2_656 ?
O4 P1 O2 Be1 76.0(6) . . . 2_656 ?
O4 P1 O1 Be2 98.3(9) . . . . ?
O4 P2 O7 P3 61.6(5) . . . . ?
O4 P2 O5 Be3 -71.9(18) . . . 1_655 ?
O4 P2 O6 Be1 167.6(5) . . . . ?
O8 P3 O9 Be3 86.6(5) . . . . ?
O8 P3 O10 P4 5.0(5) . . . . ?
O8 P3 O7 P2 -27.1(6) . . . . ?
O7 P3 O9 Be3 -151.7(5) . . . . ?
O7 P3 O10 P4 -112.6(5) . . . . ?
O7 P3 O8 Be3 79.8(14) . . . 2_546 ?
O7 P2 O4 P1 87.7(5) . . . . ?
O7 P2 O5 Be3 173.1(18) . . . 1_655 ?
O7 P2 O6 Be1 -78.4(5) . . . . ?
O5 P2 O4 P1 -25.7(5) . . . . ?
O5 P2 O7 P3 178.4(5) . . . . ?
O5 P2 O6 Be1 43.3(6) . . . . ?
O6 P2 O4 P1 -157.3(4) . . . . ?
O6 P2 O7 P3 -50.3(6) . . . . ?
O6 P2 O5 Be3 49.7(19) . . . 1_655 ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_libepo4
_database_code_depnum_ccdc_archive 'CCDC 2384142'
loop_
_audit_author_name
_audit_author_address
'Xia Zhang'
;Shanxi Normal University
China
;
_audit_update_record             
;
2024-09-14 deposited with the CCDC.	2025-04-25 downloaded from the CCDC.
;
_audit_creation_date             2024-09-14
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.06(Be32 Li32 O128 P32)'
_chemical_formula_sum            'Be2 Li2 O8 P2'
_chemical_formula_weight         221.84
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Be Be 0.0005 0.0002 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           9
_space_group_name_H-M_alt        'C 1 c 1'
_space_group_name_Hall           'C -2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'

_cell_length_a                   16.3316(4)
_cell_length_b                   9.1517(2)
_cell_length_c                   15.9658(4)
_cell_angle_alpha                90
_cell_angle_beta                 111.6240(10)
_cell_angle_gamma                90
_cell_volume                     2218.34(9)
_cell_formula_units_Z            16
_cell_measurement_reflns_used    9950
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      31.53
_cell_measurement_theta_min      2.74
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    0.788
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.657
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1728
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.15
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0423
_diffrn_reflns_av_unetI/netI     0.0376
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            34591
_diffrn_reflns_point_group_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.504
_diffrn_reflns_theta_min         2.599
_diffrn_ambient_temperature      273.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.983
_reflns_Friedel_fraction_full    0.985
_reflns_Friedel_fraction_max     0.982
_reflns_number_gt                5602
_reflns_number_total             6698
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_refine_diff_density_max         0.505
_refine_diff_density_min         -0.668
_refine_diff_density_rms         0.146
_refine_ls_abs_structure_details 
;
 Flack x determined using 2409 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.02(3)
_refine_ls_extinction_coef       0.0056(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     506
_refine_ls_number_reflns         6698
_refine_ls_number_restraints     2
_refine_ls_R_factor_all          0.0316
_refine_ls_R_factor_gt           0.0261
_refine_ls_restrained_S_all      1.030
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0457P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0673
_refine_ls_wR_factor_ref         0.0717
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
P1 P 0.44704(3) 0.03215(6) 0.59700(3) 0.00465(12) Uani 1 1 d . . . . .
P2 P 0.19555(3) 0.78368(6) 0.59720(3) 0.00460(12) Uani 1 1 d . . . . .
P3 P 0.47606(3) 0.56440(6) 0.59778(3) 0.00464(12) Uani 1 1 d . . . . .
P4 P 0.51076(3) 0.78325(6) 0.34730(3) 0.00427(12) Uani 1 1 d . . . . .
P5 P 0.72727(3) -0.18767(6) 0.59714(3) 0.00450(12) Uani 1 1 d . . . . .
P6 P 0.48175(3) 0.30856(6) 0.34618(3) 0.00437(12) Uani 1 1 d . . . . .
P7 P 0.25919(3) 1.03100(6) 0.34722(3) 0.00434(11) Uani 1 1 d . . . . .
P8 P 0.23304(3) 0.56047(6) 0.34668(3) 0.00437(12) Uani 1 1 d . . . . .
O1 O 0.10811(9) 0.74561(15) 0.60821(9) 0.0077(3) Uani 1 1 d . . . . .
O2 O 0.54665(9) 0.68318(15) 0.61061(9) 0.0076(3) Uani 1 1 d . . . . .
O3 O 0.38455(9) 0.63564(15) 0.56075(9) 0.0074(3) Uani 1 1 d . . . . .
O4 O 0.63635(9) -0.11449(15) 0.56082(9) 0.0076(3) Uani 1 1 d . . . . .
O5 O 0.27971(10) 1.19463(15) 0.35475(10) 0.0081(3) Uani 1 1 d . . . . .
O6 O 0.22654(10) 0.44511(14) 0.27471(9) 0.0073(3) Uani 1 1 d . . . . .
O7 O 0.32516(10) 0.95456(14) 0.31316(9) 0.0074(3) Uani 1 1 d . . . . .
O8 O 0.43683(10) 0.18784(14) 0.55913(9) 0.0074(3) Uani 1 1 d . . . . .
O9 O 0.27040(10) 0.77637(16) 0.68921(9) 0.0080(3) Uani 1 1 d . . . . .
O10 O 0.36090(9) -0.00867(15) 0.60993(9) 0.0074(3) Uani 1 1 d . . . . .
O11 O 0.47689(10) 0.19512(14) 0.27360(9) 0.0074(3) Uani 1 1 d . . . . .
O12 O 0.57547(9) 0.70404(14) 0.31295(9) 0.0074(3) Uani 1 1 d . . . . .
O13 O 0.25710(11) 0.48353(13) 0.43821(10) 0.0074(3) Uani 1 1 d . . . . .
O14 O 0.73585(11) -0.30082(15) 0.52972(10) 0.0085(3) Uani 1 1 d . . . . .
O15 O 0.52287(10) 0.02489(15) 0.68863(9) 0.0079(3) Uani 1 1 d . . . . .
O16 O 0.54856(10) 0.43172(15) 0.35646(10) 0.0082(3) Uani 1 1 d . . . . .
O17 O 0.50833(11) 0.23058(14) 0.43717(10) 0.0082(3) Uani 1 1 d . . . . .
O18 O 0.79826(9) -0.06984(14) 0.60986(9) 0.0076(3) Uani 1 1 d . . . . .
O19 O 0.46434(10) -0.07439(15) 0.53068(10) 0.0082(3) Uani 1 1 d . . . . .
O20 O 0.51830(11) 0.72548(15) 0.44018(10) 0.0079(3) Uani 1 1 d . . . . .
O21 O 0.16618(9) 0.99480(14) 0.28000(9) 0.0076(3) Uani 1 1 d . . . . .
O22 O 0.53372(10) 0.94602(15) 0.35567(10) 0.0080(3) Uani 1 1 d . . . . .
O23 O 0.18851(10) 0.93828(14) 0.55830(9) 0.0070(3) Uani 1 1 d . . . . .
O24 O 0.14195(9) 0.63468(14) 0.31654(9) 0.0083(3) Uani 1 1 d . . . . .
O25 O 0.27090(10) 0.97307(14) 0.44079(10) 0.0077(3) Uani 1 1 d . . . . .
O26 O 0.39036(9) 0.38061(14) 0.31595(9) 0.0082(3) Uani 1 1 d . . . . .
O27 O 0.30137(10) 0.68042(16) 0.35601(10) 0.0084(3) Uani 1 1 d . . . . .
O28 O 0.48508(10) 0.45237(15) 0.53019(10) 0.0088(3) Uani 1 1 d . . . . .
O29 O 0.74196(10) -0.25890(16) 0.68790(10) 0.0082(3) Uani 1 1 d . . . . .
O30 O 0.21172(10) 0.67456(15) 0.53209(10) 0.0089(3) Uani 1 1 d . . . . .
O31 O 0.49108(10) 0.49284(16) 0.68859(9) 0.0083(3) Uani 1 1 d . . . . .
O32 O 0.41742(9) 0.74935(14) 0.27941(9) 0.0082(3) Uani 1 1 d . . . . .
Be1 Be 0.28888(18) 0.5611(3) 0.53756(18) 0.0077(5) Uani 1 1 d . . . . .
Be2 Be 0.54412(18) 0.0629(3) 0.28195(19) 0.0071(5) Uani 1 1 d . . . . .
Be3 Be 0.54146(18) -0.1901(3) 0.53682(19) 0.0070(5) Uani 1 1 d . . . . .
Be4 Be 0.29314(19) 0.3114(3) 0.28322(19) 0.0079(5) Uani 1 1 d . . . . .
Be5 Be 0.50872(19) 0.2806(3) 0.53512(19) 0.0073(5) Uani 1 1 d . . . . .
Be6 Be 0.26254(19) 1.0273(3) 0.53500(18) 0.0071(5) Uani 1 1 d . . . . .
Be7 Be 0.57210(18) 0.5337(3) 0.28479(19) 0.0069(5) Uani 1 1 d . . . . .
Be8 Be 0.32265(18) 0.7853(3) 0.28337(19) 0.0071(5) Uani 1 1 d . . . . .
Li1 Li 0.3550(4) 0.8010(4) 0.4712(3) 0.0188(8) Uani 1 1 d . . . . .
Li2 Li 0.5972(3) 0.0574(4) 0.4711(3) 0.0212(10) Uani 1 1 d . . . . .
Li3 Li 0.5740(3) 0.5297(4) 0.4773(3) 0.0158(8) Uani 1 1 d . . . . .
Li4 Li 0.6134(3) 0.1757(4) 0.7247(3) 0.0145(8) Uani 1 1 d . . . . .
Li5 Li 0.3160(3) 1.2849(4) 0.4741(3) 0.0160(8) Uani 1 1 d . . . . .
Li6 Li 0.3639(3) -0.0767(4) 0.7250(3) 0.0143(8) Uani 1 1 d . . . . .
Li7 Li 0.6412(3) 0.7020(4) 0.7251(3) 0.0138(8) Uani 1 1 d . . . . .
Li8 Li 0.8918(3) -0.0483(4) 0.7256(3) 0.0160(8) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
P1 O8 1.5327(14) . ?
P1 O10 1.5411(15) . ?
P1 O15 1.5307(15) . ?
P1 O19 1.5401(15) . ?
P1 Li1 2.923(4) 1_545 ?
P1 Li4 3.029(4) . ?
P1 Li6 3.010(4) . ?
P2 O1 1.5416(15) . ?
P2 O9 1.5274(15) . ?
P2 O23 1.5324(14) . ?
P2 O30 1.5329(15) . ?
P2 Li2 2.922(4) 3_455 ?
P2 Li4 2.989(4) 3_455 ?
P2 Li6 3.037(4) 1_565 ?
P3 O2 1.5424(15) . ?
P3 O3 1.5351(14) . ?
P3 O28 1.5345(15) . ?
P3 O31 1.5260(15) . ?
P3 Li3 2.937(4) . ?
P3 Li7 2.992(4) . ?
P3 Li8 3.032(4) 3_455 ?
P4 O12 1.5395(14) . ?
P4 O20 1.5358(15) . ?
P4 O22 1.5299(14) . ?
P4 O32 1.5419(14) . ?
P4 Li3 3.029(4) . ?
P4 Li4 3.033(4) 2_564 ?
P4 Li8 3.065(4) 4_454 ?
P5 O4 1.5346(14) . ?
P5 O14 1.5369(15) . ?
P5 O18 1.5410(15) . ?
P5 O29 1.5252(15) . ?
P5 Li5 2.849(4) 3_535 ?
P5 Li7 3.047(4) 1_545 ?
P5 Li8 2.999(4) . ?
P6 O11 1.5359(14) . ?
P6 O16 1.5349(15) . ?
P6 O17 1.5308(15) . ?
P6 O26 1.5378(15) . ?
P6 Li3 2.902(4) . ?
P6 Li6 3.034(4) 2_554 ?
P6 Li8 2.931(4) 4_454 ?
P7 O5 1.5295(14) . ?
P7 O7 1.5420(15) . ?
P7 O21 1.5386(14) . ?
P7 O25 1.5294(15) . ?
P7 Li1 2.918(4) . ?
P7 Li5 2.997(4) . ?
P7 Li6 3.060(4) 2_564 ?
P7 Li7 3.048(4) 4_464 ?
P8 O6 1.5350(14) . ?
P8 O13 1.5370(15) . ?
P8 O24 1.5422(15) . ?
P8 O27 1.5330(15) . ?
P8 Li4 3.079(4) 4_454 ?
P8 Li7 2.932(4) 4_464 ?
O1 Be5 1.644(3) 3_455 ?
O1 Li4 1.938(4) 3_455 ?
O2 Be3 1.633(3) 1_565 ?
O2 Li7 1.917(4) . ?
O3 Be1 1.618(3) . ?
O3 Li1 2.014(4) . ?
O4 Be3 1.609(3) . ?
O4 Li2 2.065(4) . ?
O5 Be4 1.637(3) 1_565 ?
O5 Li5 1.958(4) . ?
O6 Be4 1.609(3) . ?
O6 Li4 2.047(4) 4_454 ?
O7 Be8 1.616(3) . ?
O7 Li6 2.070(4) 2_564 ?
O8 Be5 1.606(3) . ?
O8 Li5 2.134(5) 1_545 ?
O9 Be4 1.620(3) 2_565 ?
O9 Li6 1.956(4) 1_565 ?
O10 Be6 1.644(3) 1_545 ?
O10 Li6 1.924(4) . ?
O11 Be2 1.606(3) . ?
O11 Li6 2.031(4) 2_554 ?
O12 Be7 1.618(3) . ?
O12 Li4 2.056(4) 2_564 ?
O13 Be1 1.638(3) . ?
O13 Li5 2.037(4) 1_545 ?
O14 Be6 1.626(3) 3_535 ?
O14 Li5 1.993(5) 3_535 ?
O15 Be2 1.614(3) 2 ?
O15 Li4 1.947(4) . ?
O16 Be7 1.628(3) . ?
O16 Li3 2.027(4) . ?
O17 Be5 1.627(3) . ?
O17 Li2 2.081(5) . ?
O18 Be1 1.631(3) 3_545 ?
O18 Li5 2.648(4) 3_535 ?
O18 Li8 1.925(5) . ?
O19 Be3 1.620(3) . ?
O19 Li1 2.035(5) 1_545 ?
O20 Be3 1.640(3) 1_565 ?
O20 Li3 1.997(4) . ?
O21 Be7 1.606(3) 3_455 ?
O21 Li7 1.978(4) 4_464 ?
O22 Be2 1.645(3) 1_565 ?
O22 Li2 2.025(5) 1_565 ?
O23 Be6 1.611(3) . ?
O23 Li3 2.022(4) 3_455 ?
O24 Be2 1.624(3) 3_455 ?
O24 Li7 2.086(4) 4_464 ?
O25 Be6 1.637(3) . ?
O25 Li1 2.028(4) . ?
O26 Be4 1.607(3) . ?
O26 Li8 2.112(4) 4_454 ?
O27 Be8 1.638(3) . ?
O27 Li1 2.045(5) . ?
O28 Be5 1.613(3) . ?
O28 Li3 2.056(5) . ?
O29 Be8 1.624(3) 4 ?
O29 Li7 1.977(4) 1_545 ?
O30 Be1 1.610(3) . ?
O30 Li2 2.062(5) 3_455 ?
O31 Be7 1.634(3) 2_565 ?
O31 Li8 1.956(4) 3_455 ?
O32 Be8 1.606(3) . ?
O32 Li8 2.009(4) 4_454 ?
Be1 Li1 2.820(5) . ?
Be1 Li2 2.912(6) 3_455 ?
Be1 Li5 2.818(4) 1_545 ?
Be1 Li8 3.020(5) 3_455 ?
Be2 Li2 2.818(5) . ?
Be2 Li4 2.765(5) 2_554 ?
Be2 Li6 2.744(5) 2_554 ?
Be2 Li7 3.005(5) 2_564 ?
Be3 Li1 2.833(6) 1_545 ?
Be3 Li2 2.787(5) . ?
Be3 Li3 2.852(5) 1_545 ?
Be3 Li7 3.010(5) 1_545 ?
Be4 Li4 2.736(5) 4_454 ?
Be4 Li5 2.941(5) 1_545 ?
Be4 Li6 2.758(5) 2_554 ?
Be4 Li8 3.039(5) 4_454 ?
Be5 Li2 2.898(5) . ?
Be5 Li3 2.813(5) . ?
Be5 Li4 3.031(5) . ?
Be5 Li5 2.933(5) 1_545 ?
Be6 Li1 2.957(5) . ?
Be6 Li3 2.871(5) 3_455 ?
Be6 Li5 2.809(5) . ?
Be6 Li6 3.025(5) 1_565 ?
Be7 Li3 3.062(5) . ?
Be7 Li4 2.988(5) 2_564 ?
Be7 Li7 2.762(5) 2_564 ?
Be7 Li8 2.744(5) 4_454 ?
Be8 Li1 2.851(6) . ?
Be8 Li6 2.982(5) 2_564 ?
Be8 Li7 2.761(5) 4_464 ?
Be8 Li8 2.757(5) 4_454 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 P1 O10 107.83(8) . . ?
O8 P1 O19 109.77(8) . . ?
O8 P1 Li1 116.63(10) . 1_545 ?
O8 P1 Li4 78.61(9) . . ?
O8 P1 Li6 124.38(10) . . ?
O10 P1 Li1 69.69(12) . 1_545 ?
O10 P1 Li4 130.65(9) . . ?
O10 P1 Li6 33.54(9) . . ?
O15 P1 O8 110.45(8) . . ?
O15 P1 O10 108.57(8) . . ?
O15 P1 O19 109.93(9) . . ?
O15 P1 Li1 130.94(11) . 1_545 ?
O15 P1 Li4 33.57(9) . . ?
O15 P1 Li6 75.23(10) . . ?
O19 P1 O10 110.26(8) . . ?
O19 P1 Li1 41.20(13) . 1_545 ?
O19 P1 Li4 113.01(10) . . ?
O19 P1 Li6 120.03(10) . . ?
Li1 P1 Li4 151.96(13) 1_545 . ?
Li1 P1 Li6 88.90(13) 1_545 . ?
Li6 P1 Li4 101.74(11) . . ?
O1 P2 Li2 67.76(12) . 3_455 ?
O1 P2 Li4 34.95(9) . 3_455 ?
O1 P2 Li6 131.75(10) . 1_565 ?
O9 P2 O1 109.09(8) . . ?
O9 P2 O23 110.13(8) . . ?
O9 P2 O30 110.30(9) . . ?
O9 P2 Li2 132.35(10) . 3_455 ?
O9 P2 Li4 74.44(10) . 3_455 ?
O9 P2 Li6 33.55(9) . 1_565 ?
O23 P2 O1 108.70(8) . . ?
O23 P2 O30 109.43(8) . . ?
O23 P2 Li2 115.77(10) . 3_455 ?
O23 P2 Li4 126.57(10) . 3_455 ?
O23 P2 Li6 78.34(9) . 1_565 ?
O30 P2 O1 109.17(8) . . ?
O30 P2 Li2 42.21(12) . 3_455 ?
O30 P2 Li4 118.62(10) . 3_455 ?
O30 P2 Li6 112.98(10) . 1_565 ?
Li2 P2 Li4 87.95(12) 3_455 3_455 ?
Li2 P2 Li6 153.24(13) 3_455 1_565 ?
Li4 P2 Li6 101.78(12) 3_455 1_565 ?
O2 P3 Li3 66.57(10) . . ?
O2 P3 Li7 33.96(9) . . ?
O2 P3 Li8 130.76(10) . 3_455 ?
O3 P3 O2 109.01(8) . . ?
O3 P3 Li3 118.76(10) . . ?
O3 P3 Li7 126.08(9) . . ?
O3 P3 Li8 77.57(10) . 3_455 ?
O28 P3 O2 107.67(8) . . ?
O28 P3 O3 110.18(8) . . ?
O28 P3 Li3 41.46(10) . . ?
O28 P3 Li7 117.57(10) . . ?
O28 P3 Li8 115.54(10) . 3_455 ?
O31 P3 O2 109.01(8) . . ?
O31 P3 O3 109.94(9) . . ?
O31 P3 O28 110.97(8) . . ?
O31 P3 Li3 129.81(10) . . ?
O31 P3 Li7 75.29(10) . . ?
O31 P3 Li8 33.75(10) . 3_455 ?
Li3 P3 Li7 85.32(12) . . ?
Li3 P3 Li8 153.63(11) . 3_455 ?
Li7 P3 Li8 101.83(12) . 3_455 ?
O12 P4 O32 106.58(8) . . ?
O12 P4 Li3 77.18(10) . . ?
O12 P4 Li4 38.14(9) . 2_564 ?
O12 P4 Li8 78.57(9) . 4_454 ?
O20 P4 O12 111.13(8) . . ?
O20 P4 O32 108.43(9) . . ?
O20 P4 Li3 35.82(10) . . ?
O20 P4 Li4 143.05(11) . 2_564 ?
O20 P4 Li8 100.20(10) . 4_454 ?
O22 P4 O12 108.13(8) . . ?
O22 P4 O20 108.72(8) . . ?
O22 P4 O32 113.85(8) . . ?
O22 P4 Li3 132.47(10) . . ?
O22 P4 Li4 76.10(9) . 2_564 ?
O22 P4 Li8 144.71(10) . 4_454 ?
O32 P4 Li3 109.06(10) . . ?
O32 P4 Li4 102.08(10) . 2_564 ?
O32 P4 Li8 35.06(9) . 4_454 ?
Li3 P4 Li4 114.04(12) . 2_564 ?
Li3 P4 Li8 82.72(11) . 4_454 ?
Li4 P4 Li8 92.84(11) 2_564 4_454 ?
O4 P5 O14 110.77(8) . . ?
O4 P5 O18 108.70(8) . . ?
O4 P5 Li5 116.42(11) . 3_535 ?
O4 P5 Li7 77.11(9) . 1_545 ?
O4 P5 Li8 124.83(9) . . ?
O14 P5 O18 107.78(8) . . ?
O14 P5 Li5 42.01(10) . 3_535 ?
O14 P5 Li7 115.47(9) . 1_545 ?
O14 P5 Li8 118.40(10) . . ?
O18 P5 Li5 66.64(10) . 3_535 ?
O18 P5 Li7 130.84(10) . 1_545 ?
O18 P5 Li8 34.02(9) . . ?
O29 P5 O4 109.70(8) . . ?
O29 P5 O14 110.76(8) . . ?
O29 P5 O18 109.06(8) . . ?
O29 P5 Li5 132.49(11) . 3_535 ?
O29 P5 Li7 34.02(10) . 1_545 ?
O29 P5 Li8 75.19(10) . . ?
Li5 P5 Li7 155.56(11) 3_535 1_545 ?
Li5 P5 Li8 87.36(12) 3_535 . ?
Li8 P5 Li7 101.58(12) . 1_545 ?
O11 P6 O26 106.18(8) . . ?
O11 P6 Li3 152.18(11) . . ?
O11 P6 Li6 37.05(9) . 2_554 ?
O11 P6 Li8 97.84(10) . 4_454 ?
O16 P6 O11 114.46(8) . . ?
O16 P6 O26 106.75(8) . . ?
O16 P6 Li3 41.52(10) . . ?
O16 P6 Li6 147.22(10) . 2_554 ?
O16 P6 Li8 71.65(9) . 4_454 ?
O17 P6 O11 108.58(8) . . ?
O17 P6 O16 107.40(9) . . ?
O17 P6 O26 113.62(9) . . ?
O17 P6 Li3 75.55(10) . . ?
O17 P6 Li6 99.80(10) . 2_554 ?
O17 P6 Li8 150.50(10) . 4_454 ?
O26 P6 Li3 96.48(10) . . ?
O26 P6 Li6 77.62(9) . 2_554 ?
O26 P6 Li8 43.90(10) . 4_454 ?
Li3 P6 Li6 170.50(13) . 2_554 ?
Li3 P6 Li8 87.30(11) . 4_454 ?
Li8 P6 Li6 93.34(12) 4_454 2_554 ?
O5 P7 O7 108.09(8) . . ?
O5 P7 O21 113.39(8) . . ?
O5 P7 Li1 127.28(11) . . ?
O5 P7 Li5 35.25(10) . . ?
O5 P7 Li6 76.03(9) . 2_564 ?
O5 P7 Li7 143.49(10) . 4_464 ?
O7 P7 Li1 69.04(12) . . ?
O7 P7 Li5 120.52(11) . . ?
O7 P7 Li6 37.80(9) . 2_564 ?
O7 P7 Li7 79.40(10) . 4_464 ?
O21 P7 O7 107.14(8) . . ?
O21 P7 Li1 117.56(11) . . ?
O21 P7 Li5 128.21(11) . . ?
O21 P7 Li6 102.99(10) . 2_564 ?
O21 P7 Li7 34.36(9) . 4_464 ?
O25 P7 O5 108.53(8) . . ?
O25 P7 O7 109.57(8) . . ?
O25 P7 O21 110.04(9) . . ?
O25 P7 Li1 40.93(12) . . ?
O25 P7 Li5 73.28(9) . . ?
O25 P7 Li6 140.52(10) . 2_564 ?
O25 P7 Li7 101.79(9) . 4_464 ?
Li1 P7 Li5 98.39(13) . . ?
Li1 P7 Li6 104.18(14) . 2_564 ?
Li1 P7 Li7 89.07(10) . 4_464 ?
Li5 P7 Li6 102.63(11) . 2_564 ?
Li5 P7 Li7 160.07(12) . 4_464 ?
Li7 P7 Li6 93.31(11) 4_464 2_564 ?
O6 P8 O13 108.64(8) . . ?
O6 P8 O24 106.06(8) . . ?
O6 P8 Li4 36.00(9) . 4_454 ?
O6 P8 Li7 97.87(9) . 4_464 ?
O13 P8 O24 112.18(9) . . ?
O13 P8 Li4 99.23(9) . 4_454 ?
O13 P8 Li7 149.12(10) . 4_464 ?
O24 P8 Li4 78.30(9) . 4_454 ?
O24 P8 Li7 42.93(10) . 4_464 ?
O27 P8 O6 114.34(8) . . ?
O27 P8 O13 108.29(9) . . ?
O27 P8 O24 107.40(8) . . ?
O27 P8 Li4 146.48(10) . 4_454 ?
O27 P8 Li7 73.12(10) . 4_464 ?
Li7 P8 Li4 92.92(11) 4_464 4_454 ?
P2 O1 Be5 126.07(12) . 3_455 ?
P2 O1 Li4 117.95(15) . 3_455 ?
Be5 O1 Li4 115.36(17) 3_455 3_455 ?
P3 O2 Be3 124.56(14) . 1_565 ?
P3 O2 Li7 119.35(14) . . ?
Be3 O2 Li7 115.69(17) 1_565 . ?
P3 O3 Be1 129.05(13) . . ?
P3 O3 Li1 122.48(18) . . ?
Be1 O3 Li1 101.3(2) . . ?
P5 O4 Be3 127.98(13) . . ?
P5 O4 Li2 127.14(17) . . ?
Be3 O4 Li2 97.91(19) . . ?
P7 O5 Be4 131.79(13) . 1_565 ?
P7 O5 Li5 117.95(14) . . ?
Be4 O5 Li5 109.46(16) 1_565 . ?
P8 O6 Be4 126.98(14) . . ?
P8 O6 Li4 117.85(14) . 4_454 ?
Be4 O6 Li4 96.17(16) . 4_454 ?
P7 O7 Be8 126.39(14) . . ?
P7 O7 Li6 115.04(13) . 2_564 ?
Be8 O7 Li6 107.35(16) . 2_564 ?
P1 O8 Be5 127.08(14) . . ?
P1 O8 Li5 125.36(14) . 1_545 ?
Be5 O8 Li5 102.37(17) . 1_545 ?
P2 O9 Be4 137.86(14) . 2_565 ?
P2 O9 Li6 120.88(15) . 1_565 ?
Be4 O9 Li6 100.51(17) 2_565 1_565 ?
P1 O10 Be6 123.32(12) . 1_545 ?
P1 O10 Li6 120.19(15) . . ?
Be6 O10 Li6 115.73(17) 1_545 . ?
P6 O11 Be2 127.08(14) . . ?
P6 O11 Li6 115.84(14) . 2_554 ?
Be2 O11 Li6 97.27(16) . 2_554 ?
P4 O12 Be7 126.53(13) . . ?
P4 O12 Li4 114.32(13) . 2_564 ?
Be7 O12 Li4 108.27(16) . 2_564 ?
P8 O13 Be1 126.95(12) . . ?
P8 O13 Li5 127.22(15) . 1_545 ?
Be1 O13 Li5 99.55(17) . 1_545 ?
P5 O14 Be6 135.01(14) . 3_535 ?
P5 O14 Li5 106.92(14) . 3_535 ?
Be6 O14 Li5 101.34(17) 3_535 3_535 ?
P1 O15 Be2 136.62(14) . 2 ?
P1 O15 Li4 120.67(15) . . ?
Be2 O15 Li4 101.46(17) 2 . ?
P6 O16 Be7 133.48(13) . . ?
P6 O16 Li3 108.35(15) . . ?
Be7 O16 Li3 113.37(16) . . ?
P6 O17 Be5 132.85(13) . . ?
P6 O17 Li2 121.89(16) . . ?
Be5 O17 Li2 102.07(18) . . ?
P5 O18 Be1 123.42(14) . 3_545 ?
P5 O18 Li5 81.07(11) . 3_535 ?
P5 O18 Li8 119.37(14) . . ?
Be1 O18 Li5 78.44(13) 3_545 3_535 ?
Be1 O18 Li8 116.00(17) 3_545 . ?
Li8 O18 Li5 123.35(17) . 3_535 ?
P1 O19 Be3 135.02(15) . . ?
P1 O19 Li1 108.90(17) . 1_545 ?
Be3 O19 Li1 101.00(17) . 1_545 ?
P4 O20 Be3 130.89(13) . 1_565 ?
P4 O20 Li3 117.44(15) . . ?
Be3 O20 Li3 102.80(17) 1_565 . ?
P7 O21 Be7 129.42(14) . 3_455 ?
P7 O21 Li7 119.61(15) . 4_464 ?
Be7 O21 Li7 100.26(17) 3_455 4_464 ?
P4 O22 Be2 131.10(13) . 1_565 ?
P4 O22 Li2 126.62(15) . 1_565 ?
Be2 O22 Li2 99.80(17) 1_565 1_565 ?
P2 O23 Be6 127.59(14) . . ?
P2 O23 Li3 123.71(15) . 3_455 ?
Be6 O23 Li3 103.83(17) . 3_455 ?
P8 O24 Be2 130.01(12) . 3_455 ?
P8 O24 Li7 106.84(14) . 4_464 ?
Be2 O24 Li7 107.50(17) 3_455 4_464 ?
P7 O25 Be6 140.33(12) . . ?
P7 O25 Li1 109.46(17) . . ?
Be6 O25 Li1 107.10(18) . . ?
P6 O26 Be4 131.41(13) . . ?
P6 O26 Li8 105.79(14) . 4_454 ?
Be4 O26 Li8 108.80(17) . 4_454 ?
P8 O27 Be8 133.43(14) . . ?
P8 O27 Li1 121.93(17) . . ?
Be8 O27 Li1 100.86(17) . . ?
P3 O28 Be5 134.41(14) . . ?
P3 O28 Li3 108.91(14) . . ?
Be5 O28 Li3 99.39(16) . . ?
P5 O29 Be8 138.11(14) . 4 ?
P5 O29 Li7 120.40(15) . 1_545 ?
Be8 O29 Li7 99.69(17) 4 1_545 ?
P2 O30 Be1 135.26(15) . . ?
P2 O30 Li2 107.84(16) . 3_455 ?
Be1 O30 Li2 104.21(17) . 3_455 ?
P3 O31 Be7 138.38(14) . 2_565 ?
P3 O31 Li8 120.57(16) . 3_455 ?
Be7 O31 Li8 99.31(18) 2_565 3_455 ?
P4 O32 Be8 130.43(14) . . ?
P4 O32 Li8 118.77(15) . 4_454 ?
Be8 O32 Li8 98.78(16) . 4_454 ?
O3 Be1 O13 109.82(18) . . ?
O3 Be1 O18 108.47(17) . 3_455 ?
O3 Be1 Li1 44.46(13) . . ?
O3 Be1 Li2 154.98(17) . 3_455 ?
O3 Be1 Li5 101.20(16) . 1_545 ?
O3 Be1 Li8 77.03(13) . 3_455 ?
O13 Be1 Li1 90.12(15) . . ?
O13 Be1 Li2 74.18(14) . 3_455 ?
O13 Be1 Li5 45.48(12) . 1_545 ?
O13 Be1 Li8 132.91(15) . 3_455 ?
O18 Be1 O13 106.30(16) 3_455 . ?
O18 Be1 Li1 152.69(19) 3_455 . ?
O18 Be1 Li2 93.30(15) 3_455 3_455 ?
O18 Be1 Li5 67.01(13) 3_455 1_545 ?
O18 Be1 Li8 34.96(11) 3_455 3_455 ?
O30 Be1 O3 114.26(17) . . ?
O30 Be1 O13 105.34(17) . . ?
O30 Be1 O18 112.31(18) . 3_455 ?
O30 Be1 Li1 82.99(15) . . ?
O30 Be1 Li2 43.36(12) . 3_455 ?
O30 Be1 Li5 141.48(18) . 1_545 ?
O30 Be1 Li8 113.91(16) . 3_455 ?
Li1 Be1 Li2 112.40(16) . 3_455 ?
Li1 Be1 Li8 118.79(16) . 3_455 ?
Li2 Be1 Li8 119.23(15) 3_455 3_455 ?
Li5 Be1 Li1 115.51(16) 1_545 . ?
Li5 Be1 Li2 98.55(15) 1_545 3_455 ?
Li5 Be1 Li8 87.51(13) 1_545 3_455 ?
O11 Be2 O15 113.00(19) . 2_554 ?
O11 Be2 O22 107.56(17) . 1_545 ?
O11 Be2 O24 106.28(15) . 3_545 ?
O11 Be2 Li2 91.92(15) . . ?
O11 Be2 Li4 156.61(19) . 2_554 ?
O11 Be2 Li6 47.24(12) . 2_554 ?
O11 Be2 Li7 81.74(13) . 2_564 ?
O15 Be2 O22 107.03(15) 2_554 1_545 ?
O15 Be2 O24 111.41(18) 2_554 3_545 ?
O15 Be2 Li2 148.95(17) 2_554 . ?
O15 Be2 Li4 43.65(12) 2_554 2_554 ?
O15 Be2 Li6 82.98(15) 2_554 2_554 ?
O15 Be2 Li7 92.03(15) 2_554 2_564 ?
O22 Be2 Li2 45.08(12) 1_545 . ?
O22 Be2 Li4 83.44(13) 1_545 2_554 ?
O22 Be2 Li6 83.45(15) 1_545 2_554 ?
O22 Be2 Li7 152.49(17) 1_545 2_564 ?
O24 Be2 O22 111.57(18) 3_545 1_545 ?
O24 Be2 Li2 76.54(15) 3_545 . ?
O24 Be2 Li4 87.75(14) 3_545 2_554 ?
O24 Be2 Li6 153.44(16) 3_545 2_554 ?
O24 Be2 Li7 41.47(11) 3_545 2_564 ?
Li2 Be2 Li7 110.38(15) . 2_564 ?
Li4 Be2 Li2 109.78(15) 2_554 . ?
Li4 Be2 Li7 98.03(14) 2_554 2_564 ?
Li6 Be2 Li2 102.98(17) 2_554 . ?
Li6 Be2 Li4 116.49(16) 2_554 2_554 ?
Li6 Be2 Li7 119.23(15) 2_554 2_564 ?
O2 Be3 O20 106.05(16) 1_545 1_545 ?
O2 Be3 Li1 90.52(15) 1_545 1_545 ?
O2 Be3 Li2 155.76(18) 1_545 . ?
O2 Be3 Li3 68.61(13) 1_545 1_545 ?
O2 Be3 Li7 35.04(11) 1_545 1_545 ?
O4 Be3 O2 110.13(18) . 1_545 ?
O4 Be3 O19 113.12(17) . . ?
O4 Be3 O20 107.13(17) . 1_545 ?
O4 Be3 Li1 155.53(17) . 1_545 ?
O4 Be3 Li2 47.21(13) . . ?
O4 Be3 Li3 100.64(15) . 1_545 ?
O4 Be3 Li7 77.51(14) . 1_545 ?
O19 Be3 O2 109.89(17) . 1_545 ?
O19 Be3 O20 110.26(18) . 1_545 ?
O19 Be3 Li1 44.84(12) . 1_545 ?
O19 Be3 Li2 78.52(15) . . ?
O19 Be3 Li3 143.44(18) . 1_545 ?
O19 Be3 Li7 113.42(16) . 1_545 ?
O20 Be3 Li1 78.16(15) 1_545 1_545 ?
O20 Be3 Li2 91.30(15) 1_545 . ?
O20 Be3 Li3 43.07(12) 1_545 1_545 ?
O20 Be3 Li7 129.58(15) 1_545 1_545 ?
Li1 Be3 Li3 99.05(14) 1_545 1_545 ?
Li1 Be3 Li7 118.19(16) 1_545 1_545 ?
Li2 Be3 Li1 109.89(16) . 1_545 ?
Li2 Be3 Li3 118.58(16) . 1_545 ?
Li2 Be3 Li7 120.75(16) . 1_545 ?
Li3 Be3 Li7 86.51(13) 1_545 1_545 ?
O5 Be4 Li4 82.17(15) 1_545 4_454 ?
O5 Be4 Li5 38.88(11) 1_545 1_545 ?
O5 Be4 Li6 84.65(14) 1_545 2_554 ?
O5 Be4 Li8 154.08(18) 1_545 4_454 ?
O6 Be4 O5 107.17(18) . 1_545 ?
O6 Be4 O9 112.45(18) . 2_564 ?
O6 Be4 Li4 48.05(12) . 4_454 ?
O6 Be4 Li5 88.50(15) . 1_545 ?
O6 Be4 Li6 156.64(19) . 2_554 ?
O6 Be4 Li8 81.34(13) . 4_454 ?
O9 Be4 O5 106.17(16) 2_564 1_545 ?
O9 Be4 Li4 81.61(15) 2_564 4_454 ?
O9 Be4 Li5 144.81(16) 2_564 1_545 ?
O9 Be4 Li6 44.21(12) 2_564 2_554 ?
O9 Be4 Li8 92.26(15) 2_564 4_454 ?
O26 Be4 O5 113.62(18) . 1_545 ?
O26 Be4 O6 106.50(16) . . ?
O26 Be4 O9 110.99(18) . 2_564 ?
O26 Be4 Li4 154.33(17) . 4_454 ?
O26 Be4 Li5 87.86(15) . 1_545 ?
O26 Be4 Li6 85.98(15) . 2_554 ?
O26 Be4 Li8 41.15(12) . 4_454 ?
Li4 Be4 Li5 93.90(15) 4_454 1_545 ?
Li4 Be4 Li6 116.66(16) 4_454 2_554 ?
Li4 Be4 Li8 119.19(15) 4_454 4_454 ?
Li5 Be4 Li8 119.59(15) 1_545 4_454 ?
Li6 Be4 Li5 112.08(14) 2_554 1_545 ?
Li6 Be4 Li8 96.83(14) 2_554 4_454 ?
O1 Be5 Li2 67.84(14) 3_545 . ?
O1 Be5 Li3 89.81(14) 3_545 . ?
O1 Be5 Li4 35.29(11) 3_545 . ?
O1 Be5 Li5 153.71(17) 3_545 1_545 ?
O8 Be5 O1 110.18(17) . 3_545 ?
O8 Be5 O17 109.65(17) . . ?
O8 Be5 O28 110.12(18) . . ?
O8 Be5 Li2 102.42(15) . . ?
O8 Be5 Li3 154.94(18) . . ?
O8 Be5 Li4 77.70(13) . . ?
O8 Be5 Li5 45.30(12) . 1_545 ?
O17 Be5 O1 106.28(17) . 3_545 ?
O17 Be5 Li2 44.62(12) . . ?
O17 Be5 Li3 77.32(14) . . ?
O17 Be5 Li4 132.16(16) . . ?
O17 Be5 Li5 93.49(15) . 1_545 ?
O28 Be5 O1 112.36(17) . 3_545 ?
O28 Be5 O17 108.13(17) . . ?
O28 Be5 Li2 144.19(17) . . ?
O28 Be5 Li3 46.14(12) . . ?
O28 Be5 Li4 113.21(16) . . ?
O28 Be5 Li5 76.26(14) . 1_545 ?
Li2 Be5 Li4 87.59(13) . . ?
Li2 Be5 Li5 120.41(15) . 1_545 ?
Li3 Be5 Li2 99.03(15) . . ?
Li3 Be5 Li4 116.24(15) . . ?
Li3 Be5 Li5 111.73(14) . 1_545 ?
Li5 Be5 Li4 118.50(14) 1_545 . ?
O10 Be6 Li1 67.92(14) 1_565 . ?
O10 Be6 Li3 151.63(17) 1_565 3_455 ?
O10 Be6 Li5 94.31(16) 1_565 . ?
O10 Be6 Li6 34.95(11) 1_565 1_565 ?
O14 Be6 O10 113.76(18) 3_465 1_565 ?
O14 Be6 O25 110.93(17) 3_465 . ?
O14 Be6 Li1 145.18(17) 3_465 . ?
O14 Be6 Li3 74.96(14) 3_465 3_455 ?
O14 Be6 Li5 44.08(12) 3_465 . ?
O14 Be6 Li6 113.18(16) 3_465 1_565 ?
O23 Be6 O10 110.23(17) . 1_565 ?
O23 Be6 O14 106.96(17) . 3_465 ?
O23 Be6 O25 112.50(18) . . ?
O23 Be6 Li1 104.31(15) . . ?
O23 Be6 Li3 43.16(12) . 3_455 ?
O23 Be6 Li5 149.28(18) . . ?
O23 Be6 Li6 77.84(13) . 1_565 ?
O25 Be6 O10 102.58(17) . 1_565 ?
O25 Be6 Li1 40.96(12) . . ?
O25 Be6 Li3 98.64(16) . 3_455 ?
O25 Be6 Li5 78.15(13) . . ?
O25 Be6 Li6 128.76(16) . 1_565 ?
Li1 Be6 Li6 87.98(13) . 1_565 ?
Li3 Be6 Li1 121.23(16) 3_455 . ?
Li3 Be6 Li6 116.77(15) 3_455 1_565 ?
Li5 Be6 Li1 101.86(15) . . ?
Li5 Be6 Li3 108.40(15) . 3_455 ?
Li5 Be6 Li6 119.09(16) . 1_565 ?
O12 Be7 O16 110.45(17) . . ?
O12 Be7 O31 109.70(17) . 2_564 ?
O12 Be7 Li3 75.26(13) . . ?
O12 Be7 Li4 40.78(11) . 2_564 ?
O12 Be7 Li7 150.69(17) . 2_564 ?
O12 Be7 Li8 88.34(14) . 4_454 ?
O16 Be7 O31 104.86(16) . 2_564 ?
O16 Be7 Li3 37.41(11) . . ?
O16 Be7 Li4 151.09(16) . 2_564 ?
O16 Be7 Li7 91.57(14) . 2_564 ?
O16 Be7 Li8 76.63(14) . 4_454 ?
O21 Be7 O12 106.94(17) 3_545 . ?
O21 Be7 O16 112.60(17) 3_545 . ?
O21 Be7 O31 112.32(18) 3_545 2_564 ?
O21 Be7 Li3 112.91(16) 3_545 . ?
O21 Be7 Li4 81.30(14) 3_545 2_564 ?
O21 Be7 Li7 44.83(12) 3_545 2_564 ?
O21 Be7 Li8 156.68(18) 3_545 4_454 ?
O31 Be7 Li3 130.29(17) 2_564 . ?
O31 Be7 Li4 91.75(15) 2_564 2_564 ?
O31 Be7 Li7 81.50(14) 2_564 2_564 ?
O31 Be7 Li8 44.70(13) 2_564 4_454 ?
Li4 Be7 Li3 114.38(13) 2_564 . ?
Li7 Be7 Li3 118.88(15) 2_564 . ?
Li7 Be7 Li4 114.52(15) 2_564 2_564 ?
Li8 Be7 Li3 87.63(14) 4_454 . ?
Li8 Be7 Li4 100.74(14) 4_454 2_564 ?
Li8 Be7 Li7 116.27(15) 4_454 2_564 ?
O7 Be8 O27 110.01(17) . . ?
O7 Be8 O29 110.03(17) . 4_454 ?
O7 Be8 Li1 70.58(13) . . ?
O7 Be8 Li6 41.50(11) . 2_564 ?
O7 Be8 Li7 88.08(14) . 4_464 ?
O7 Be8 Li8 152.06(18) . 4_454 ?
O27 Be8 Li1 44.78(12) . . ?
O27 Be8 Li6 151.19(17) . 2_564 ?
O27 Be8 Li7 77.41(14) . 4_464 ?
O27 Be8 Li8 89.75(14) . 4_454 ?
O29 Be8 O27 105.47(17) 4_454 . ?
O29 Be8 Li1 140.05(19) 4_454 . ?
O29 Be8 Li6 92.21(15) 4_454 2_564 ?
O29 Be8 Li7 44.88(12) 4_454 4_464 ?
O29 Be8 Li8 81.93(14) 4_454 4_454 ?
O32 Be8 O7 106.72(17) . . ?
O32 Be8 O27 111.51(17) . . ?
O32 Be8 O29 113.14(18) . 4_454 ?
O32 Be8 Li1 104.12(18) . . ?
O32 Be8 Li6 80.73(14) . 2_564 ?
O32 Be8 Li7 157.69(18) . 4_464 ?
O32 Be8 Li8 46.06(12) . 4_454 ?
Li1 Be8 Li6 107.94(14) . 2_564 ?
Li7 Be8 Li1 96.44(16) 4_464 . ?
Li7 Be8 Li6 101.25(14) 4_464 2_564 ?
Li8 Be8 Li1 116.85(16) 4_454 . ?
Li8 Be8 Li6 115.56(15) 4_454 2_564 ?
Li8 Be8 Li7 116.19(15) 4_454 4_464 ?
P1 Li1 Be6 56.96(9) 1_565 . ?
P7 Li1 P1 87.44(10) . 1_565 ?
P7 Li1 Be6 60.92(9) . . ?
O3 Li1 P1 97.36(18) . 1_565 ?
O3 Li1 P7 162.1(3) . . ?
O3 Li1 O19 98.7(2) . 1_565 ?
O3 Li1 O25 135.8(3) . . ?
O3 Li1 O27 98.30(17) . . ?
O3 Li1 Be1 34.24(10) . . ?
O3 Li1 Be3 79.38(17) . 1_565 ?
O3 Li1 Be6 107.5(2) . . ?
O3 Li1 Be8 127.73(18) . . ?
O19 Li1 P1 29.90(7) 1_565 1_565 ?
O19 Li1 P7 94.07(14) 1_565 . ?
O19 Li1 O27 137.2(3) 1_565 . ?
O19 Li1 Be1 130.8(2) 1_565 . ?
O19 Li1 Be3 34.16(11) 1_565 1_565 ?
O19 Li1 Be6 85.31(14) 1_565 . ?
O19 Li1 Be8 108.0(2) 1_565 . ?
O25 Li1 P1 74.56(12) . 1_565 ?
O25 Li1 P7 29.61(8) . . ?
O25 Li1 O19 94.40(16) . 1_565 ?
O25 Li1 O27 100.1(2) . . ?
O25 Li1 Be1 112.0(2) . . ?
O25 Li1 Be3 127.37(19) . 1_565 ?
O25 Li1 Be6 31.95(10) . . ?
O25 Li1 Be8 86.58(17) . . ?
O27 Li1 P1 161.8(2) . 1_565 ?
O27 Li1 P7 80.45(15) . . ?
O27 Li1 Be1 79.71(15) . . ?
O27 Li1 Be3 113.2(2) . 1_565 ?
O27 Li1 Be6 125.7(2) . . ?
O27 Li1 Be8 34.36(10) . . ?
Be1 Li1 P1 118.47(18) . 1_565 ?
Be1 Li1 P7 129.2(2) . . ?
Be1 Li1 Be3 113.08(16) . 1_565 ?
Be1 Li1 Be6 95.80(18) . . ?
Be1 Li1 Be8 114.07(16) . . ?
Be3 Li1 P1 60.96(11) 1_565 1_565 ?
Be3 Li1 P7 117.68(17) 1_565 . ?
Be3 Li1 Be6 117.92(16) 1_565 . ?
Be3 Li1 Be8 98.49(19) 1_565 . ?
Be8 Li1 P1 127.46(17) . 1_565 ?
Be8 Li1 P7 58.49(10) . . ?
Be8 Li1 Be6 118.51(16) . . ?
O4 Li2 P2 96.35(17) . 3_545 ?
O4 Li2 O17 140.2(3) . . ?
O4 Li2 Be1 74.89(16) . 3_545 ?
O4 Li2 Be2 130.67(19) . . ?
O4 Li2 Be3 34.88(10) . . ?
O4 Li2 Be5 111.1(2) . . ?
O17 Li2 P2 78.06(13) . 3_545 ?
O17 Li2 Be1 129.7(2) . 3_545 ?
O17 Li2 Be2 78.35(15) . . ?
O17 Li2 Be3 115.0(2) . . ?
O17 Li2 Be5 33.31(10) . . ?
O22 Li2 P2 162.0(2) 1_545 3_545 ?
O22 Li2 O4 99.89(18) 1_545 . ?
O22 Li2 O17 94.2(2) 1_545 . ?
O22 Li2 O30 139.7(3) 1_545 3_545 ?
O22 Li2 Be1 117.3(2) 1_545 3_545 ?
O22 Li2 Be2 35.12(10) 1_545 . ?
O22 Li2 Be3 78.75(15) 1_545 . ?
O22 Li2 Be5 121.4(2) 1_545 . ?
O30 Li2 P2 29.96(7) 3_545 3_545 ?
O30 Li2 O4 94.2(2) 3_545 . ?
O30 Li2 O17 98.69(18) 3_545 . ?
O30 Li2 Be1 32.42(10) 3_545 3_545 ?
O30 Li2 Be2 111.4(2) 3_545 . ?
O30 Li2 Be3 127.6(2) 3_545 . ?
O30 Li2 Be5 87.14(15) 3_545 . ?
Be1 Li2 P2 59.77(11) 3_545 3_545 ?
Be2 Li2 P2 126.85(17) . 3_545 ?
Be2 Li2 Be1 104.80(18) . 3_545 ?
Be2 Li2 Be5 111.65(16) . . ?
Be3 Li2 P2 119.28(17) . 3_545 ?
Be3 Li2 Be1 109.18(16) . 3_545 ?
Be3 Li2 Be2 113.83(17) . . ?
Be3 Li2 Be5 99.51(18) . . ?
Be5 Li2 P2 58.41(10) . 3_545 ?
Be5 Li2 Be1 118.17(16) . 3_545 ?
P3 Li3 P4 103.64(12) . . ?
P3 Li3 Be7 148.18(17) . . ?
P4 Li3 Be7 55.16(9) . . ?
P6 Li3 P3 106.54(14) . . ?
P6 Li3 P4 94.87(12) . . ?
P6 Li3 Be7 58.25(9) . . ?
O16 Li3 P3 134.5(2) . . ?
O16 Li3 P4 77.79(13) . . ?
O16 Li3 P6 30.13(8) . . ?
O16 Li3 O28 108.1(2) . . ?
O16 Li3 Be3 135.83(19) . 1_565 ?
O16 Li3 Be5 89.10(16) . . ?
O16 Li3 Be6 96.96(17) . 3_545 ?
O16 Li3 Be7 29.22(9) . . ?
O20 Li3 P3 78.42(14) . . ?
O20 Li3 P4 26.74(8) . . ?
O20 Li3 P6 110.68(18) . . ?
O20 Li3 O16 101.75(19) . . ?
O20 Li3 O23 140.7(2) . 3_545 ?
O20 Li3 O28 96.76(19) . . ?
O20 Li3 Be3 34.12(10) . 1_565 ?
O20 Li3 Be5 129.7(2) . . ?
O20 Li3 Be6 114.79(19) . 3_545 ?
O20 Li3 Be7 81.77(15) . . ?
O23 Li3 P3 102.96(16) 3_545 . ?
O23 Li3 P4 139.2(2) 3_545 . ?
O23 Li3 P6 106.52(15) 3_545 . ?
O23 Li3 O16 104.01(19) 3_545 . ?
O23 Li3 O28 102.79(19) 3_545 . ?
O23 Li3 Be3 113.63(19) 3_545 1_565 ?
O23 Li3 Be5 80.07(14) 3_545 . ?
O23 Li3 Be6 33.02(10) 3_545 3_545 ?
O23 Li3 Be7 108.15(18) 3_545 . ?
O28 Li3 P3 29.62(7) . . ?
O28 Li3 P4 115.56(18) . . ?
O28 Li3 P6 78.39(14) . . ?
O28 Li3 Be3 85.78(15) . 1_565 ?
O28 Li3 Be5 34.47(9) . . ?
O28 Li3 Be6 134.57(19) . 3_545 ?
O28 Li3 Be7 132.0(2) . . ?
Be3 Li3 P3 58.09(9) 1_565 . ?
Be3 Li3 P4 58.76(9) 1_565 . ?
Be3 Li3 P6 139.18(17) 1_565 . ?
Be3 Li3 Be6 102.08(15) 1_565 3_545 ?
Be3 Li3 Be7 112.94(15) 1_565 . ?
Be5 Li3 P3 60.59(10) . . ?
Be5 Li3 P4 140.45(18) . . ?
Be5 Li3 P6 60.84(10) . . ?
Be5 Li3 Be3 118.67(17) . 1_565 ?
Be5 Li3 Be6 112.31(15) . 3_545 ?
Be5 Li3 Be7 118.30(16) . . ?
Be6 Li3 P3 124.69(16) 3_545 . ?
Be6 Li3 P4 106.27(14) 3_545 . ?
Be6 Li3 P6 115.86(14) 3_545 . ?
Be6 Li3 Be7 86.27(14) 3_545 . ?
P1 Li4 P4 85.20(10) . 2_565 ?
P1 Li4 P8 108.91(12) . 4 ?
P1 Li4 Be5 55.24(9) . . ?
P2 Li4 P1 101.64(12) 3_545 . ?
P2 Li4 P4 153.13(14) 3_545 2_565 ?
P2 Li4 P8 108.86(13) 3_545 4 ?
P2 Li4 Be5 56.29(9) 3_545 . ?
P4 Li4 P8 92.94(11) 2_565 4 ?
O1 Li4 P1 77.65(14) 3_545 . ?
O1 Li4 P2 27.11(7) 3_545 3_545 ?
O1 Li4 P4 137.62(19) 3_545 2_565 ?
O1 Li4 P8 129.21(18) 3_545 4 ?
O1 Li4 O6 105.50(19) 3_545 4 ?
O1 Li4 O12 124.3(2) 3_545 2_565 ?
O1 Li4 O15 101.0(2) 3_545 . ?
O1 Li4 Be2 134.4(2) 3_545 2 ?
O1 Li4 Be4 88.63(16) 3_545 4 ?
O1 Li4 Be5 29.35(10) 3_545 . ?
O1 Li4 Be7 94.52(16) 3_545 2_565 ?
O6 Li4 P1 119.04(17) 4 . ?
O6 Li4 P2 82.93(13) 4 3_545 ?
O6 Li4 P4 116.68(16) 4 2_565 ?
O6 Li4 P8 26.15(7) 4 4 ?
O6 Li4 O12 118.6(2) 4 2_565 ?
O6 Li4 Be2 82.24(14) 4 2 ?
O6 Li4 Be4 35.78(10) 4 4 ?
O6 Li4 Be5 131.06(18) 4 . ?
O6 Li4 Be7 129.31(19) 4 2_565 ?
O12 Li4 P1 105.76(16) 2_565 . ?
O12 Li4 P2 127.89(17) 2_565 3_545 ?
O12 Li4 P4 27.55(7) 2_565 2_565 ?
O12 Li4 P8 102.90(15) 2_565 4 ?
O12 Li4 Be2 86.15(15) 2_565 2 ?
O12 Li4 Be4 107.39(18) 2_565 4 ?
O12 Li4 Be5 108.27(16) 2_565 . ?
O12 Li4 Be7 30.95(9) 2_565 2_565 ?
O15 Li4 P1 25.76(8) . . ?
O15 Li4 P2 121.04(18) . 3_545 ?
O15 Li4 P4 74.86(13) . 2_565 ?
O15 Li4 P8 85.71(14) . 4 ?
O15 Li4 O6 102.15(18) . 4 ?
O15 Li4 O12 101.22(19) . 2_565 ?
O15 Li4 Be2 34.90(10) . 2 ?
O15 Li4 Be4 137.2(2) . 4 ?
O15 Li4 Be5 80.93(15) . . ?
O15 Li4 Be7 119.29(18) . 2_565 ?
Be2 Li4 P1 60.37(10) 2 . ?
Be2 Li4 P2 145.84(16) 2 3_545 ?
Be2 Li4 P4 59.59(10) 2 2_565 ?
Be2 Li4 P8 58.54(10) 2 4 ?
Be2 Li4 Be5 115.57(16) 2 . ?
Be2 Li4 Be7 115.37(16) 2 2_565 ?
Be4 Li4 P1 146.29(16) 4 . ?
Be4 Li4 P2 61.56(10) 4 3_545 ?
Be4 Li4 P4 123.54(16) 4 2_565 ?
Be4 Li4 P8 57.52(10) 4 4 ?
Be4 Li4 Be2 116.05(16) 4 2 ?
Be4 Li4 Be5 117.82(15) 4 . ?
Be4 Li4 Be7 101.10(15) 4 2_565 ?
Be5 Li4 P4 111.27(14) . 2_565 ?
Be5 Li4 P8 147.89(15) . 4 ?
Be7 Li4 P1 110.47(14) 2_565 . ?
Be7 Li4 P2 97.78(12) 2_565 3_545 ?
Be7 Li4 P4 55.85(9) 2_565 2_565 ?
Be7 Li4 P8 125.96(15) 2_565 4 ?
Be7 Li4 Be5 85.85(12) 2_565 . ?
P5 Li5 P7 115.16(14) 3_465 . ?
P5 Li5 Be4 143.59(18) 3_465 1_565 ?
P5 Li5 Be5 121.90(16) 3_465 1_565 ?
O5 Li5 P5 131.3(2) . 3_465 ?
O5 Li5 P7 26.80(7) . . ?
O5 Li5 O8 108.69(19) . 1_565 ?
O5 Li5 O13 99.2(2) . 1_565 ?
O5 Li5 O14 104.8(2) . 3_465 ?
O5 Li5 O18 157.5(2) . 3_465 ?
O5 Li5 Be1 134.2(2) . 1_565 ?
O5 Li5 Be4 31.66(9) . 1_565 ?
O5 Li5 Be5 102.73(18) . 1_565 ?
O5 Li5 Be6 87.79(15) . . ?
O8 Li5 P5 100.61(16) 1_565 3_465 ?
O8 Li5 P7 95.19(14) 1_565 . ?
O8 Li5 O18 92.45(16) 1_565 3_465 ?
O8 Li5 Be1 112.07(18) 1_565 1_565 ?
O8 Li5 Be4 115.34(18) 1_565 1_565 ?
O8 Li5 Be5 32.33(9) 1_565 1_565 ?
O8 Li5 Be6 76.28(14) 1_565 . ?
O13 Li5 P5 78.95(14) 1_565 3_465 ?
O13 Li5 P7 120.35(19) 1_565 . ?
O13 Li5 O8 141.3(2) 1_565 1_565 ?
O13 Li5 O18 66.41(12) 1_565 3_465 ?
O13 Li5 Be1 34.97(9) 1_565 1_565 ?
O13 Li5 Be4 76.61(14) 1_565 1_565 ?
O13 Li5 Be5 116.29(18) 1_565 1_565 ?
O13 Li5 Be6 132.2(2) 1_565 . ?
O14 Li5 P5 31.07(8) 3_465 3_465 ?
O14 Li5 P7 84.57(14) 3_465 . ?
O14 Li5 O8 99.08(18) 3_465 1_565 ?
O14 Li5 O13 99.1(2) 3_465 1_565 ?
O14 Li5 O18 62.96(12) 3_465 3_465 ?
O14 Li5 Be1 88.69(16) 3_465 1_565 ?
O14 Li5 Be4 129.8(2) 3_465 1_565 ?
O14 Li5 Be5 130.3(2) 3_465 1_565 ?
O14 Li5 Be6 34.58(9) 3_465 . ?
O18 Li5 P5 32.30(6) 3_465 3_465 ?
O18 Li5 P7 147.44(17) 3_465 . ?
O18 Li5 Be1 34.56(8) 3_465 1_565 ?
O18 Li5 Be4 142.81(16) 3_465 1_565 ?
O18 Li5 Be5 99.35(15) 3_465 1_565 ?
O18 Li5 Be6 89.79(14) 3_465 . ?
Be1 Li5 P5 59.07(10) 1_565 3_465 ?
Be1 Li5 P7 152.64(19) 1_565 . ?
Be1 Li5 Be4 108.78(14) 1_565 1_565 ?
Be1 Li5 Be5 100.61(15) 1_565 1_565 ?
Be4 Li5 P7 58.26(9) 1_565 . ?
Be5 Li5 P7 103.95(14) 1_565 . ?
Be5 Li5 Be4 93.21(14) 1_565 1_565 ?
Be6 Li5 P5 62.19(10) . 3_465 ?
Be6 Li5 P7 61.63(10) . . ?
Be6 Li5 Be1 121.22(17) . 1_565 ?
Be6 Li5 Be4 119.41(16) . 1_565 ?
Be6 Li5 Be5 107.83(15) . 1_565 ?
P1 Li6 P2 101.89(12) . 1_545 ?
P1 Li6 P6 109.00(13) . 2 ?
P1 Li6 P7 152.34(14) . 2_565 ?
P1 Li6 Be6 55.38(9) . 1_545 ?
P2 Li6 P7 84.57(10) 1_545 2_565 ?
P6 Li6 P2 109.78(12) 2 1_545 ?
P6 Li6 P7 93.52(11) 2 2_565 ?
O7 Li6 P1 127.63(16) 2_565 . ?
O7 Li6 P2 104.82(16) 2_565 1_545 ?
O7 Li6 P6 103.03(16) 2_565 2 ?
O7 Li6 P7 27.16(7) 2_565 2_565 ?
O7 Li6 Be2 108.04(18) 2_565 2 ?
O7 Li6 Be4 85.44(15) 2_565 2 ?
O7 Li6 Be6 108.68(16) 2_565 1_545 ?
O7 Li6 Be8 31.15(9) 2_565 2_565 ?
O9 Li6 P1 121.86(18) 1_545 . ?
O9 Li6 P2 25.57(7) 1_545 1_545 ?
O9 Li6 P6 87.07(14) 1_545 2 ?
O9 Li6 P7 73.77(13) 1_545 2_565 ?
O9 Li6 O7 99.70(19) 1_545 2_565 ?
O9 Li6 O11 104.25(18) 1_545 2 ?
O9 Li6 Be2 139.02(19) 1_545 2 ?
O9 Li6 Be4 35.28(10) 1_545 2 ?
O9 Li6 Be6 80.97(15) 1_545 1_545 ?
O9 Li6 Be8 117.65(19) 1_545 2_565 ?
O10 Li6 P1 26.27(8) . . ?
O10 Li6 P2 78.22(14) . 1_545 ?
O10 Li6 P6 128.48(19) . 2 ?
O10 Li6 P7 137.84(19) . 2_565 ?
O10 Li6 O7 124.6(2) . 2_565 ?
O10 Li6 O9 101.6(2) . 1_545 ?
O10 Li6 O11 103.7(2) . 2 ?
O10 Li6 Be2 87.05(16) . 2 ?
O10 Li6 Be4 135.0(2) . 2 ?
O10 Li6 Be6 29.32(10) . 1_545 ?
O10 Li6 Be8 94.59(15) . 2_565 ?
O11 Li6 P1 82.09(14) 2 . ?
O11 Li6 P2 120.12(16) 2 1_545 ?
O11 Li6 P6 27.10(7) 2 2 ?
O11 Li6 P7 118.16(17) 2 2_565 ?
O11 Li6 O7 119.4(2) 2 2_565 ?
O11 Li6 Be2 35.49(9) 2 2 ?
O11 Li6 Be4 83.69(14) 2 2 ?
O11 Li6 Be6 129.44(19) 2 1_545 ?
O11 Li6 Be8 129.50(19) 2 2_565 ?
Be2 Li6 P1 60.84(10) 2 . ?
Be2 Li6 P2 146.79(16) 2 1_545 ?
Be2 Li6 P6 58.00(10) 2 2 ?
Be2 Li6 P7 124.46(16) 2 2_565 ?
Be2 Li6 Be4 117.11(16) 2 2 ?
Be2 Li6 Be6 116.20(16) 2 1_545 ?
Be2 Li6 Be8 101.18(14) 2 2_565 ?
Be4 Li6 P1 146.76(16) 2 . ?
Be4 Li6 P2 60.68(10) 2 1_545 ?
Be4 Li6 P6 59.10(10) 2 2 ?
Be4 Li6 P7 59.31(10) 2 2_565 ?
Be4 Li6 Be6 116.12(16) 2 1_545 ?
Be4 Li6 Be8 114.85(16) 2 2_565 ?
Be6 Li6 P2 55.45(9) 1_545 1_545 ?
Be6 Li6 P6 147.52(15) 1_545 2 ?
Be6 Li6 P7 111.62(14) 1_545 2_565 ?
Be8 Li6 P1 97.28(12) 2_565 . ?
Be8 Li6 P2 109.46(14) 2_565 1_545 ?
Be8 Li6 P6 126.13(15) 2_565 2 ?
Be8 Li6 P7 55.60(9) 2_565 2_565 ?
Be8 Li6 Be6 85.92(12) 2_565 1_545 ?
P3 Li7 P5 101.94(12) . 1_565 ?
P3 Li7 P7 109.83(12) . 4_565 ?
P3 Li7 Be2 93.58(13) . 2_565 ?
P3 Li7 Be3 55.86(9) . 1_565 ?
P5 Li7 P7 108.77(13) 1_565 4_565 ?
P8 Li7 P3 151.02(15) 4_565 . ?
P8 Li7 P5 87.05(10) 4_565 1_565 ?
P8 Li7 P7 92.68(12) 4_565 4_565 ?
P8 Li7 Be2 57.81(9) 4_565 2_565 ?
P8 Li7 Be3 111.99(13) 4_565 1_565 ?
O2 Li7 P3 26.70(8) . . ?
O2 Li7 P5 78.40(14) . 1_565 ?
O2 Li7 P7 130.11(17) . 4_565 ?
O2 Li7 P8 137.18(18) . 4_565 ?
O2 Li7 O21 107.6(2) . 4_565 ?
O2 Li7 O24 121.7(2) . 4_565 ?
O2 Li7 O29 101.36(19) . 1_565 ?
O2 Li7 Be2 91.30(16) . 2_565 ?
O2 Li7 Be3 29.28(9) . 1_565 ?
O2 Li7 Be7 88.32(16) . 2_565 ?
O2 Li7 Be8 135.4(2) . 4_565 ?
O21 Li7 P3 84.54(14) 4_565 . ?
O21 Li7 P5 121.88(18) 4_565 1_565 ?
O21 Li7 P7 26.03(7) 4_565 4_565 ?
O21 Li7 P8 114.21(18) 4_565 4_565 ?
O21 Li7 O24 113.3(2) 4_565 4_565 ?
O21 Li7 Be2 124.30(19) 4_565 2_565 ?
O21 Li7 Be3 133.51(19) 4_565 1_565 ?
O21 Li7 Be7 34.91(10) 4_565 2_565 ?
O21 Li7 Be8 82.47(15) 4_565 4_565 ?
O24 Li7 P3 123.23(18) 4_565 . ?
O24 Li7 P5 110.29(15) 4_565 1_565 ?
O24 Li7 P7 102.38(15) 4_565 4_565 ?
O24 Li7 P8 30.23(7) 4_565 4_565 ?
O24 Li7 Be2 31.04(9) 4_565 2_565 ?
O24 Li7 Be3 108.97(16) 4_565 1_565 ?
O24 Li7 Be7 102.45(17) 4_565 2_565 ?
O24 Li7 Be8 90.32(16) 4_565 4_565 ?
O29 Li7 P3 120.91(18) 1_565 . ?
O29 Li7 P5 25.58(7) 1_565 1_565 ?
O29 Li7 P7 85.36(14) 1_565 4_565 ?
O29 Li7 P8 77.62(13) 1_565 4_565 ?
O29 Li7 O21 103.86(19) 1_565 4_565 ?
O29 Li7 O24 106.85(19) 1_565 4_565 ?
O29 Li7 Be2 123.47(17) 1_565 2_565 ?
O29 Li7 Be3 81.06(14) 1_565 1_565 ?
O29 Li7 Be7 137.43(19) 1_565 2_565 ?
O29 Li7 Be8 35.44(10) 1_565 4_565 ?
Be2 Li7 P5 112.98(13) 2_565 1_565 ?
Be2 Li7 P7 125.96(15) 2_565 4_565 ?
Be2 Li7 Be3 85.12(12) 2_565 1_565 ?
Be3 Li7 P5 55.61(9) 1_565 1_565 ?
Be3 Li7 P7 148.26(15) 1_565 4_565 ?
Be7 Li7 P3 61.63(10) 2_565 . ?
Be7 Li7 P5 146.97(16) 2_565 1_565 ?
Be7 Li7 P7 58.36(9) 2_565 4_565 ?
Be7 Li7 P8 121.67(15) 2_565 4_565 ?
Be7 Li7 Be2 97.27(15) 2_565 2_565 ?
Be7 Li7 Be3 117.46(16) 2_565 1_565 ?
Be8 Li7 P3 146.44(16) 4_565 . ?
Be8 Li7 P5 60.61(10) 4_565 1_565 ?
Be8 Li7 P7 57.81(9) 4_565 4_565 ?
Be8 Li7 P8 61.47(10) 4_565 4_565 ?
Be8 Li7 Be2 119.23(16) 4_565 2_565 ?
Be8 Li7 Be3 116.19(16) 4_565 1_565 ?
Be8 Li7 Be7 116.17(16) 4_565 2_565 ?
P3 Li8 P4 109.05(13) 3_545 4 ?
P3 Li8 Be4 112.58(13) 3_545 4 ?
P5 Li8 P3 101.47(13) . 3_545 ?
P5 Li8 P4 109.52(12) . 4 ?
P5 Li8 Be1 55.31(9) . 3_545 ?
P5 Li8 Be4 93.96(13) . 4 ?
P6 Li8 P3 86.87(10) 4 3_545 ?
P6 Li8 P4 93.53(12) 4 4 ?
P6 Li8 P5 150.86(15) 4 . ?
P6 Li8 Be1 111.43(13) 4 3_545 ?
P6 Li8 Be4 57.36(9) 4 4 ?
O18 Li8 P3 77.60(14) . 3_545 ?
O18 Li8 P4 129.06(17) . 4 ?
O18 Li8 P5 26.61(8) . . ?
O18 Li8 P6 137.34(18) . 4 ?
O18 Li8 O26 121.7(2) . 4 ?
O18 Li8 O31 100.5(2) . 3_545 ?
O18 Li8 O32 106.5(2) . 4 ?
O18 Li8 Be1 29.05(9) . 3_545 ?
O18 Li8 Be4 92.41(16) . 4 ?
O18 Li8 Be7 135.0(2) . 4 ?
O18 Li8 Be8 87.86(16) . 4 ?
O26 Li8 P3 109.55(15) 4 3_545 ?
O26 Li8 P4 103.93(16) 4 4 ?
O26 Li8 P5 122.92(17) 4 . ?
O26 Li8 P6 30.32(7) 4 4 ?
O26 Li8 Be1 107.22(16) 4 3_545 ?
O26 Li8 Be4 30.05(9) 4 4 ?
O26 Li8 Be7 90.57(16) 4 4 ?
O26 Li8 Be8 103.54(17) 4 4 ?
O31 Li8 P3 25.68(8) 3_545 3_545 ?
O31 Li8 P4 85.65(14) 3_545 4 ?
O31 Li8 P5 120.59(19) 3_545 . ?
O31 Li8 P6 77.51(13) 3_545 4 ?
O31 Li8 O26 106.59(19) 3_545 4 ?
O31 Li8 O32 103.90(19) 3_545 4 ?
O31 Li8 Be1 81.70(15) 3_545 3_545 ?
O31 Li8 Be4 123.04(17) 3_545 4 ?
O31 Li8 Be7 35.99(10) 3_545 4 ?
O31 Li8 Be8 137.72(19) 3_545 4 ?
O32 Li8 P3 121.66(18) 4 3_545 ?
O32 Li8 P4 26.17(7) 4 4 ?
O32 Li8 P5 84.02(14) 4 . ?
O32 Li8 P6 115.45(18) 4 4 ?
O32 Li8 O26 115.2(2) 4 4 ?
O32 Li8 Be1 132.9(2) 4 3_545 ?
O32 Li8 Be4 125.04(19) 4 4 ?
O32 Li8 Be7 82.50(15) 4 4 ?
O32 Li8 Be8 35.16(10) 4 4 ?
Be1 Li8 P3 56.12(9) 3_545 3_545 ?
Be1 Li8 P4 148.58(16) 3_545 4 ?
Be1 Li8 Be4 84.35(12) 3_545 4 ?
Be4 Li8 P4 126.27(15) 4 4 ?
Be7 Li8 P3 61.29(10) 4 3_545 ?
Be7 Li8 P4 57.78(10) 4 4 ?
Be7 Li8 P5 146.47(17) 4 . ?
Be7 Li8 P6 61.50(10) 4 4 ?
Be7 Li8 Be1 117.36(16) 4 3_545 ?
Be7 Li8 Be4 118.84(16) 4 4 ?
Be7 Li8 Be8 116.30(16) 4 4 ?
Be8 Li8 P3 146.77(17) 4 3_545 ?
Be8 Li8 P4 58.53(10) 4 4 ?
Be8 Li8 P5 61.30(10) 4 . ?
Be8 Li8 P6 122.49(16) 4 4 ?
Be8 Li8 Be1 116.55(17) 4 3_545 ?
Be8 Li8 Be4 97.57(15) 4 4 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
P1 O8 Be5 O1 -36.1(2) . . . 3_545 ?
P1 O8 Be5 O17 80.5(2) . . . . ?
P1 O8 Be5 O28 -160.64(13) . . . . ?
P1 O8 Be5 Li2 34.5(2) . . . . ?
P1 O8 Be5 Li3 -177.2(3) . . . . ?
P1 O8 Be5 Li4 -50.17(16) . . . . ?
P1 O8 Be5 Li5 155.3(2) . . . 1_545 ?
P1 O19 Be3 O2 61.9(3) . . . 1_545 ?
P1 O19 Be3 O4 -61.6(3) . . . . ?
P1 O19 Be3 O20 178.46(14) . . . 1_545 ?
P1 O19 Be3 Li1 131.4(3) . . . 1_545 ?
P1 O19 Be3 Li2 -94.43(19) . . . . ?
P1 O19 Be3 Li3 142.5(2) . . . 1_545 ?
P1 O19 Be3 Li7 24.3(3) . . . 1_545 ?
P2 O23 Be6 O10 -36.5(2) . . . 1_565 ?
P2 O23 Be6 O14 -160.60(13) . . . 3_465 ?
P2 O23 Be6 O25 77.4(2) . . . . ?
P2 O23 Be6 Li1 34.9(2) . . . . ?
P2 O23 Be6 Li3 155.6(2) . . . 3_455 ?
P2 O23 Be6 Li5 -177.4(3) . . . . ?
P2 O23 Be6 Li6 -49.80(16) . . . 1_565 ?
P2 O30 Be1 O3 -59.2(3) . . . . ?
P2 O30 Be1 O13 -179.82(14) . . . . ?
P2 O30 Be1 O18 64.9(3) . . . 3_455 ?
P2 O30 Be1 Li1 -91.6(2) . . . . ?
P2 O30 Be1 Li2 134.8(3) . . . 3_455 ?
P2 O30 Be1 Li5 145.5(2) . . . 1_545 ?
P2 O30 Be1 Li8 26.8(3) . . . 3_455 ?
P3 O3 Be1 O13 -81.5(2) . . . . ?
P3 O3 Be1 O18 34.3(2) . . . 3_455 ?
P3 O3 Be1 O30 160.45(13) . . . . ?
P3 O3 Be1 Li1 -150.1(2) . . . . ?
P3 O3 Be1 Li2 -176.4(3) . . . 3_455 ?
P3 O3 Be1 Li5 -35.0(2) . . . 1_545 ?
P3 O3 Be1 Li8 49.81(16) . . . 3_455 ?
P3 O28 Be5 O1 -62.1(3) . . . 3_545 ?
P3 O28 Be5 O8 61.2(3) . . . . ?
P3 O28 Be5 O17 -179.04(14) . . . . ?
P3 O28 Be5 Li2 -144.8(2) . . . . ?
P3 O28 Be5 Li3 -128.5(2) . . . . ?
P3 O28 Be5 Li4 -23.7(3) . . . . ?
P3 O28 Be5 Li5 91.77(19) . . . 1_545 ?
P4 O12 Be7 O16 -42.0(2) . . . . ?
P4 O12 Be7 O21 -164.87(12) . . . 3_545 ?
P4 O12 Be7 O31 73.1(2) . . . 2_564 ?
P4 O12 Be7 Li3 -54.95(16) . . . . ?
P4 O12 Be7 Li4 141.6(2) . . . 2_564 ?
P4 O12 Be7 Li7 -178.4(3) . . . 2_564 ?
P4 O12 Be7 Li8 33.04(18) . . . 4_454 ?
P4 O32 Be8 O7 47.0(2) . . . . ?
P4 O32 Be8 O27 -73.2(2) . . . . ?
P4 O32 Be8 O29 168.12(12) . . . 4_454 ?
P4 O32 Be8 Li1 -26.6(2) . . . . ?
P4 O32 Be8 Li6 79.68(17) . . . 2_564 ?
P4 O32 Be8 Li7 176.7(3) . . . 4_464 ?
P4 O32 Be8 Li8 -140.5(2) . . . 4_454 ?
P5 O4 Be3 O2 38.4(2) . . . 1_545 ?
P5 O4 Be3 O19 161.79(13) . . . . ?
P5 O4 Be3 O20 -76.5(2) . . . 1_545 ?
P5 O4 Be3 Li1 -175.6(4) . . . 1_545 ?
P5 O4 Be3 Li2 -151.8(2) . . . . ?
P5 O4 Be3 Li3 -32.5(2) . . . 1_545 ?
P5 O4 Be3 Li7 51.42(16) . . . 1_545 ?
P6 O11 Be2 O15 -174.65(13) . . . 2_554 ?
P6 O11 Be2 O22 67.4(2) . . . 1_545 ?
P6 O11 Be2 O24 -52.2(2) . . . 3_545 ?
P6 O11 Be2 Li2 24.37(18) . . . . ?
P6 O11 Be2 Li4 -177.1(4) . . . 2_554 ?
P6 O11 Be2 Li6 130.33(19) . . . 2_554 ?
P6 O11 Be2 Li7 -85.95(15) . . . 2_564 ?
P6 O16 Be7 O12 131.10(17) . . . . ?
P6 O16 Be7 O21 -109.4(2) . . . 3_545 ?
P6 O16 Be7 O31 13.0(3) . . . 2_564 ?
P6 O16 Be7 Li3 152.0(3) . . . . ?
P6 O16 Be7 Li4 136.1(3) . . . 2_564 ?
P6 O16 Be7 Li7 -68.6(2) . . . 2_564 ?
P6 O16 Be7 Li8 48.02(18) . . . 4_454 ?
P6 O17 Be5 O1 -128.09(17) . . . 3_545 ?
P6 O17 Be5 O8 112.83(19) . . . . ?
P6 O17 Be5 O28 -7.3(3) . . . . ?
P6 O17 Be5 Li2 -159.3(3) . . . . ?
P6 O17 Be5 Li3 -42.1(2) . . . . ?
P6 O17 Be5 Li4 -156.13(16) . . . . ?
P6 O17 Be5 Li5 69.4(2) . . . 1_545 ?
P6 O26 Be4 O5 54.4(3) . . . 1_545 ?
P6 O26 Be4 O6 172.16(12) . . . . ?
P6 O26 Be4 O9 -65.1(2) . . . 2_564 ?
P6 O26 Be4 Li4 178.9(3) . . . 4_454 ?
P6 O26 Be4 Li5 84.36(17) . . . 1_545 ?
P6 O26 Be4 Li6 -28.0(2) . . . 2_554 ?
P6 O26 Be4 Li8 -133.1(2) . . . 4_454 ?
P7 O7 Be8 O27 -43.9(2) . . . . ?
P7 O7 Be8 O29 71.9(2) . . . 4_454 ?
P7 O7 Be8 O32 -165.04(12) . . . . ?
P7 O7 Be8 Li1 -65.58(17) . . . . ?
P7 O7 Be8 Li6 141.4(2) . . . 2_564 ?
P7 O7 Be8 Li7 31.93(18) . . . 4_464 ?
P7 O7 Be8 Li8 -176.5(3) . . . 4_454 ?
P7 O25 Be6 O10 -124.1(2) . . . 1_565 ?
P7 O25 Be6 O14 -2.3(3) . . . 3_465 ?
P7 O25 Be6 O23 117.5(2) . . . . ?
P7 O25 Be6 Li1 -156.5(3) . . . . ?
P7 O25 Be6 Li3 74.8(2) . . . 3_455 ?
P7 O25 Be6 Li5 -32.3(2) . . . . ?
P7 O25 Be6 Li6 -150.24(17) . . . 1_565 ?
P8 O6 Be4 O5 70.0(2) . . . 1_545 ?
P8 O6 Be4 O9 -173.67(13) . . . 2_564 ?
P8 O6 Be4 O26 -51.9(2) . . . . ?
P8 O6 Be4 Li4 132.04(19) . . . 4_454 ?
P8 O6 Be4 Li5 35.43(17) . . . 1_545 ?
P8 O6 Be4 Li6 -172.0(4) . . . 2_554 ?
P8 O6 Be4 Li8 -84.81(16) . . . 4_454 ?
P8 O13 Be1 O3 -67.1(2) . . . . ?
P8 O13 Be1 O18 175.74(14) . . . 3_455 ?
P8 O13 Be1 O30 56.4(2) . . . . ?
P8 O13 Be1 Li1 -26.4(2) . . . . ?
P8 O13 Be1 Li2 86.92(17) . . . 3_455 ?
P8 O13 Be1 Li5 -153.4(2) . . . 1_545 ?
P8 O13 Be1 Li8 -157.64(16) . . . 3_455 ?
P8 O27 Be8 O7 127.79(17) . . . . ?
P8 O27 Be8 O29 9.2(3) . . . 4_454 ?
P8 O27 Be8 O32 -114.0(2) . . . . ?
P8 O27 Be8 Li1 157.4(3) . . . . ?
P8 O27 Be8 Li6 135.1(3) . . . 2_564 ?
P8 O27 Be8 Li7 44.56(19) . . . 4_464 ?
P8 O27 Be8 Li8 -72.4(2) . . . 4_454 ?
O1 P2 O9 Be4 29.0(2) . . . 2_565 ?
O1 P2 O9 Li6 -138.84(17) . . . 1_565 ?
O1 P2 O23 Be6 179.78(16) . . . . ?
O1 P2 O23 Li3 -29.05(18) . . . 3_455 ?
O1 P2 O30 Be1 -122.18(19) . . . . ?
O1 P2 O30 Li2 11.54(16) . . . 3_455 ?
O2 P3 O3 Be1 -178.54(16) . . . . ?
O2 P3 O3 Li1 36.85(19) . . . . ?
O2 P3 O28 Be5 117.5(2) . . . . ?
O2 P3 O28 Li3 -7.78(17) . . . . ?
O2 P3 O31 Be7 -24.7(2) . . . 2_565 ?
O2 P3 O31 Li8 136.67(16) . . . 3_455 ?
O3 P3 O2 Be3 -45.19(17) . . . 1_565 ?
O3 P3 O2 Li7 127.12(16) . . . . ?
O3 P3 O28 Be5 -123.75(19) . . . . ?
O3 P3 O28 Li3 110.99(15) . . . . ?
O3 P3 O31 Be7 -144.2(2) . . . 2_565 ?
O3 P3 O31 Li8 17.23(18) . . . 3_455 ?
O4 P5 O14 Be6 -126.6(2) . . . 3_535 ?
O4 P5 O14 Li5 106.85(16) . . . 3_535 ?
O4 P5 O18 Be1 -41.73(17) . . . 3_545 ?
O4 P5 O18 Li5 -111.43(11) . . . 3_535 ?
O4 P5 O18 Li8 125.19(16) . . . . ?
O4 P5 O29 Be8 -143.6(2) . . . 4 ?
O4 P5 O29 Li7 17.50(18) . . . 1_545 ?
O5 P7 O7 Be8 -172.20(16) . . . . ?
O5 P7 O7 Li6 -33.33(16) . . . 2_564 ?
O5 P7 O21 Be7 -66.14(18) . . . 3_455 ?
O5 P7 O21 Li7 156.77(16) . . . 4_464 ?
O5 P7 O25 Be6 30.1(3) . . . . ?
O5 P7 O25 Li1 -126.06(16) . . . . ?
O6 P8 O13 Be1 167.99(16) . . . . ?
O6 P8 O13 Li5 21.7(2) . . . 1_545 ?
O6 P8 O24 Be2 47.38(19) . . . 3_455 ?
O6 P8 O24 Li7 -84.25(14) . . . 4_464 ?
O6 P8 O27 Be8 48.8(2) . . . . ?
O6 P8 O27 Li1 -157.63(17) . . . . ?
O7 P7 O5 Be4 50.9(2) . . . 1_565 ?
O7 P7 O5 Li5 -117.61(18) . . . . ?
O7 P7 O21 Be7 174.68(15) . . . 3_455 ?
O7 P7 O21 Li7 37.59(18) . . . 4_464 ?
O7 P7 O25 Be6 147.9(2) . . . . ?
O7 P7 O25 Li1 -8.24(18) . . . . ?
O8 P1 O10 Be6 43.56(17) . . . 1_545 ?
O8 P1 O10 Li6 -126.06(16) . . . . ?
O8 P1 O15 Be2 145.15(19) . . . 2 ?
O8 P1 O15 Li4 -19.41(19) . . . . ?
O8 P1 O19 Be3 122.88(19) . . . . ?
O8 P1 O19 Li1 -108.22(16) . . . 1_545 ?
O9 P2 O1 Be5 162.73(15) . . . 3_455 ?
O9 P2 O1 Li4 -7.77(17) . . . 3_455 ?
O9 P2 O23 Be6 60.32(19) . . . . ?
O9 P2 O23 Li3 -148.51(17) . . . 3_455 ?
O9 P2 O30 Be1 -2.3(2) . . . . ?
O9 P2 O30 Li2 131.39(15) . . . 3_455 ?
O10 P1 O8 Be5 179.27(16) . . . . ?
O10 P1 O8 Li5 -30.77(18) . . . 1_545 ?
O10 P1 O15 Be2 27.1(2) . . . 2 ?
O10 P1 O15 Li4 -137.44(16) . . . . ?
O10 P1 O19 Be3 -118.48(19) . . . . ?
O10 P1 O19 Li1 10.43(17) . . . 1_545 ?
O11 P6 O16 Be7 44.9(2) . . . . ?
O11 P6 O16 Li3 -162.16(14) . . . . ?
O11 P6 O17 Be5 -167.87(18) . . . . ?
O11 P6 O17 Li2 36.2(2) . . . . ?
O11 P6 O26 Be4 49.7(2) . . . . ?
O11 P6 O26 Li8 -84.44(14) . . . 4_454 ?
O12 P4 O20 Be3 121.68(17) . . . 1_565 ?
O12 P4 O20 Li3 -19.58(19) . . . . ?
O12 P4 O22 Be2 54.2(2) . . . 1_565 ?
O12 P4 O22 Li2 -104.2(2) . . . 1_565 ?
O12 P4 O32 Be8 172.48(16) . . . . ?
O12 P4 O32 Li8 38.34(18) . . . 4_454 ?
O13 P8 O6 Be4 -43.53(18) . . . . ?
O13 P8 O6 Li4 79.84(17) . . . 4_454 ?
O13 P8 O24 Be2 -71.08(18) . . . 3_455 ?
O13 P8 O24 Li7 157.29(13) . . . 4_464 ?
O13 P8 O27 Be8 170.02(18) . . . . ?
O13 P8 O27 Li1 -36.4(2) . . . . ?
O14 P5 O4 Be3 61.98(18) . . . . ?
O14 P5 O4 Li2 -82.13(19) . . . . ?
O14 P5 O18 Be1 78.39(16) . . . 3_545 ?
O14 P5 O18 Li5 8.69(12) . . . 3_535 ?
O14 P5 O18 Li8 -114.69(17) . . . . ?
O14 P5 O29 Be8 93.8(2) . . . 4 ?
O14 P5 O29 Li7 -105.09(17) . . . 1_545 ?
O15 P1 O8 Be5 60.78(19) . . . . ?
O15 P1 O8 Li5 -149.26(16) . . . 1_545 ?
O15 P1 O10 Be6 163.25(14) . . . 1_545 ?
O15 P1 O10 Li6 -6.37(18) . . . . ?
O15 P1 O19 Be3 1.2(2) . . . . ?
O15 P1 O19 Li1 130.10(16) . . . 1_545 ?
O16 P6 O11 Be2 78.67(17) . . . . ?
O16 P6 O11 Li6 -158.49(15) . . . 2_554 ?
O16 P6 O17 Be5 67.9(2) . . . . ?
O16 P6 O17 Li2 -88.10(19) . . . . ?
O16 P6 O26 Be4 172.19(17) . . . . ?
O16 P6 O26 Li8 38.08(15) . . . 4_454 ?
O17 P6 O11 Be2 -41.30(18) . . . . ?
O17 P6 O11 Li6 81.54(17) . . . 2_554 ?
O17 P6 O16 Be7 165.51(18) . . . . ?
O17 P6 O16 Li3 -41.53(16) . . . . ?
O17 P6 O26 Be4 -69.61(19) . . . . ?
O17 P6 O26 Li8 156.29(13) . . . 4_454 ?
O18 P5 O4 Be3 -179.77(16) . . . . ?
O18 P5 O4 Li2 36.1(2) . . . . ?
O18 P5 O14 Be6 114.6(2) . . . 3_535 ?
O18 P5 O14 Li5 -11.95(17) . . . 3_535 ?
O18 P5 O29 Be8 -24.7(2) . . . 4 ?
O18 P5 O29 Li7 136.45(16) . . . 1_545 ?
O19 P1 O8 Be5 -60.58(18) . . . . ?
O19 P1 O8 Li5 89.37(18) . . . 1_545 ?
O19 P1 O10 Be6 -76.27(16) . . . 1_545 ?
O19 P1 O10 Li6 114.11(17) . . . . ?
O19 P1 O15 Be2 -93.6(2) . . . 2 ?
O19 P1 O15 Li4 101.87(17) . . . . ?
O20 P4 O12 Be7 66.77(18) . . . . ?
O20 P4 O12 Li4 -153.51(15) . . . 2_564 ?
O20 P4 O22 Be2 175.00(17) . . . 1_565 ?
O20 P4 O22 Li2 16.6(2) . . . 1_565 ?
O20 P4 O32 Be8 52.76(18) . . . . ?
O20 P4 O32 Li8 -81.38(17) . . . 4_454 ?
O21 P7 O5 Be4 -67.8(2) . . . 1_565 ?
O21 P7 O5 Li5 123.75(18) . . . . ?
O21 P7 O7 Be8 -49.66(18) . . . . ?
O21 P7 O7 Li6 89.21(16) . . . 2_564 ?
O21 P7 O25 Be6 -94.5(2) . . . . ?
O21 P7 O25 Li1 109.33(17) . . . . ?
O22 P4 O12 Be7 -173.97(16) . . . . ?
O22 P4 O12 Li4 -34.26(16) . . . 2_564 ?
O22 P4 O20 Be3 2.8(2) . . . 1_565 ?
O22 P4 O20 Li3 -138.48(17) . . . . ?
O22 P4 O32 Be8 -68.39(19) . . . . ?
O22 P4 O32 Li8 157.47(16) . . . 4_454 ?
O23 P2 O1 Be5 42.62(17) . . . 3_455 ?
O23 P2 O1 Li4 -127.87(16) . . . 3_455 ?
O23 P2 O9 Be4 148.2(2) . . . 2_565 ?
O23 P2 O9 Li6 -19.6(2) . . . 1_565 ?
O23 P2 O30 Be1 118.97(19) . . . . ?
O23 P2 O30 Li2 -107.31(15) . . . 3_455 ?
O24 P8 O6 Be4 -164.31(15) . . . . ?
O24 P8 O6 Li4 -40.94(17) . . . 4_454 ?
O24 P8 O13 Be1 -75.08(19) . . . . ?
O24 P8 O13 Li5 138.62(19) . . . 1_545 ?
O24 P8 O27 Be8 -68.6(2) . . . . ?
O24 P8 O27 Li1 84.99(19) . . . . ?
O25 P7 O5 Be4 169.63(18) . . . 1_565 ?
O25 P7 O5 Li5 1.2(2) . . . . ?
O25 P7 O7 Be8 69.70(18) . . . . ?
O25 P7 O7 Li6 -151.43(15) . . . 2_564 ?
O25 P7 O21 Be7 55.62(18) . . . 3_455 ?
O25 P7 O21 Li7 -81.47(17) . . . 4_464 ?
O26 P6 O11 Be2 -163.83(15) . . . . ?
O26 P6 O11 Li6 -40.99(17) . . . 2_554 ?
O26 P6 O16 Be7 -72.29(19) . . . . ?
O26 P6 O16 Li3 80.67(15) . . . . ?
O26 P6 O17 Be5 -50.0(2) . . . . ?
O26 P6 O17 Li2 154.08(17) . . . . ?
O27 P8 O6 Be4 77.55(18) . . . . ?
O27 P8 O6 Li4 -159.09(16) . . . 4_454 ?
O27 P8 O13 Be1 43.3(2) . . . . ?
O27 P8 O13 Li5 -103.0(2) . . . 1_545 ?
O27 P8 O24 Be2 170.05(17) . . . 3_455 ?
O27 P8 O24 Li7 38.42(14) . . . 4_464 ?
O28 P3 O2 Be3 74.33(16) . . . 1_565 ?
O28 P3 O2 Li7 -113.36(17) . . . . ?
O28 P3 O3 Be1 63.51(18) . . . . ?
O28 P3 O3 Li1 -81.10(18) . . . . ?
O28 P3 O31 Be7 93.7(2) . . . 2_565 ?
O28 P3 O31 Li8 -104.92(17) . . . 3_455 ?
O29 P5 O4 Be3 -60.60(19) . . . . ?
O29 P5 O4 Li2 155.29(18) . . . . ?
O29 P5 O14 Be6 -4.7(2) . . . 3_535 ?
O29 P5 O14 Li5 -131.19(16) . . . 3_535 ?
O29 P5 O18 Be1 -161.30(15) . . . 3_545 ?
O29 P5 O18 Li5 129.00(12) . . . 3_535 ?
O29 P5 O18 Li8 5.62(18) . . . . ?
O30 P2 O1 Be5 -76.68(17) . . . 3_455 ?
O30 P2 O1 Li4 112.83(16) . . . 3_455 ?
O30 P2 O9 Be4 -90.9(2) . . . 2_565 ?
O30 P2 O9 Li6 101.26(17) . . . 1_565 ?
O30 P2 O23 Be6 -61.08(18) . . . . ?
O30 P2 O23 Li3 90.08(18) . . . 3_455 ?
O31 P3 O2 Be3 -165.21(15) . . . 1_565 ?
O31 P3 O2 Li7 7.10(19) . . . . ?
O31 P3 O3 Be1 -59.11(19) . . . . ?
O31 P3 O3 Li1 156.28(17) . . . . ?
O31 P3 O28 Be5 -1.7(2) . . . . ?
O31 P3 O28 Li3 -127.00(15) . . . . ?
O32 P4 O12 Be7 -51.19(17) . . . . ?
O32 P4 O12 Li4 88.53(16) . . . 2_564 ?
O32 P4 O20 Be3 -121.49(18) . . . 1_565 ?
O32 P4 O20 Li3 97.25(18) . . . . ?
O32 P4 O22 Be2 -64.0(2) . . . 1_565 ?
O32 P4 O22 Li2 137.6(2) . . . 1_565 ?
Li1 P1 O8 Be5 -105.0(2) 1_545 . . . ?
Li1 P1 O8 Li5 44.9(2) 1_545 . . 1_545 ?
Li1 P1 O10 Be6 -68.96(17) 1_545 . . 1_545 ?
Li1 P1 O10 Li6 121.42(18) 1_545 . . . ?
Li1 P1 O15 Be2 -51.7(3) 1_545 . . 2 ?
Li1 P1 O15 Li4 143.7(2) 1_545 . . . ?
Li1 P1 O19 Be3 -128.9(3) 1_545 . . . ?
Li1 P7 O5 Be4 127.9(2) . . . 1_565 ?
Li1 P7 O5 Li5 -40.6(2) . . . . ?
Li1 P7 O7 Be8 63.93(18) . . . . ?
Li1 P7 O7 Li6 -157.20(19) . . . 2_564 ?
Li1 P7 O21 Be7 99.8(2) . . . 3_455 ?
Li1 P7 O21 Li7 -37.3(2) . . . 4_464 ?
Li1 P7 O25 Be6 156.2(3) . . . . ?
Li1 O3 Be1 O13 68.7(2) . . . . ?
Li1 O3 Be1 O18 -175.56(18) . . . 3_455 ?
Li1 O3 Be1 O30 -49.4(2) . . . . ?
Li1 O3 Be1 Li2 -26.3(4) . . . 3_455 ?
Li1 O3 Be1 Li5 115.15(19) . . . 1_545 ?
Li1 O3 Be1 Li8 -160.07(17) . . . 3_455 ?
Li1 O19 Be3 O2 -69.5(2) 1_545 . . 1_545 ?
Li1 O19 Be3 O4 167.0(2) 1_545 . . . ?
Li1 O19 Be3 O20 47.0(2) 1_545 . . 1_545 ?
Li1 O19 Be3 Li2 134.2(2) 1_545 . . . ?
Li1 O19 Be3 Li3 11.1(3) 1_545 . . 1_545 ?
Li1 O19 Be3 Li7 -107.1(2) 1_545 . . 1_545 ?
Li1 O25 Be6 O10 32.4(2) . . . 1_565 ?
Li1 O25 Be6 O14 154.2(2) . . . 3_465 ?
Li1 O25 Be6 O23 -86.0(2) . . . . ?
Li1 O25 Be6 Li3 -128.68(18) . . . 3_455 ?
Li1 O25 Be6 Li5 124.2(2) . . . . ?
Li1 O25 Be6 Li6 6.3(3) . . . 1_565 ?
Li1 O27 Be8 O7 -29.6(2) . . . . ?
Li1 O27 Be8 O29 -148.24(19) . . . 4_454 ?
Li1 O27 Be8 O32 88.6(2) . . . . ?
Li1 O27 Be8 Li6 -22.4(4) . . . 2_564 ?
Li1 O27 Be8 Li7 -112.85(18) . . . 4_464 ?
Li1 O27 Be8 Li8 130.20(19) . . . 4_454 ?
Li2 P2 O1 Be5 -68.33(17) 3_455 . . 3_455 ?
Li2 P2 O1 Li4 121.18(18) 3_455 . . 3_455 ?
Li2 P2 O9 Be4 -47.9(3) 3_455 . . 2_565 ?
Li2 P2 O9 Li6 144.3(2) 3_455 . . 1_565 ?
Li2 P2 O23 Be6 -106.5(2) 3_455 . . . ?
Li2 P2 O23 Li3 44.7(2) 3_455 . . 3_455 ?
Li2 P2 O30 Be1 -133.7(3) 3_455 . . . ?
Li2 O4 Be3 O2 -169.75(18) . . . 1_545 ?
Li2 O4 Be3 O19 -46.4(2) . . . . ?
Li2 O4 Be3 O20 75.34(19) . . . 1_545 ?
Li2 O4 Be3 Li1 -23.8(5) . . . 1_545 ?
Li2 O4 Be3 Li3 119.30(18) . . . 1_545 ?
Li2 O4 Be3 Li7 -156.73(17) . . . 1_545 ?
Li2 O17 Be5 O1 31.2(2) . . . 3_545 ?
Li2 O17 Be5 O8 -87.9(2) . . . . ?
Li2 O17 Be5 O28 152.02(19) . . . . ?
Li2 O17 Be5 Li3 117.20(18) . . . . ?
Li2 O17 Be5 Li4 3.1(3) . . . . ?
Li2 O17 Be5 Li5 -131.30(17) . . . 1_545 ?
Li2 O30 Be1 O3 166.01(19) 3_455 . . . ?
Li2 O30 Be1 O13 45.4(2) 3_455 . . . ?
Li2 O30 Be1 O18 -69.9(2) 3_455 . . 3_455 ?
Li2 O30 Be1 Li1 133.6(2) 3_455 . . . ?
Li2 O30 Be1 Li5 10.8(3) 3_455 . . 1_545 ?
Li2 O30 Be1 Li8 -108.0(2) 3_455 . . 3_455 ?
Li3 P3 O2 Be3 68.72(17) . . . 1_565 ?
Li3 P3 O2 Li7 -118.97(19) . . . . ?
Li3 P3 O3 Be1 108.36(19) . . . . ?
Li3 P3 O3 Li1 -36.26(19) . . . . ?
Li3 P3 O28 Be5 125.3(3) . . . . ?
Li3 P3 O31 Be7 50.2(3) . . . 2_565 ?
Li3 P3 O31 Li8 -148.42(19) . . . 3_455 ?
Li3 P4 O12 Be7 55.17(18) . . . . ?
Li3 P4 O12 Li4 -165.11(18) . . . 2_564 ?
Li3 P4 O20 Be3 141.3(3) . . . 1_565 ?
Li3 P4 O22 Be2 143.27(19) . . . 1_565 ?
Li3 P4 O22 Li2 -15.1(3) . . . 1_565 ?
Li3 P4 O32 Be8 90.65(18) . . . . ?
Li3 P4 O32 Li8 -43.49(18) . . . 4_454 ?
Li3 P6 O11 Be2 52.9(3) . . . . ?
Li3 P6 O11 Li6 175.7(2) . . . 2_554 ?
Li3 P6 O16 Be7 -153.0(3) . . . . ?
Li3 P6 O17 Be5 40.9(2) . . . . ?
Li3 P6 O17 Li2 -115.1(2) . . . . ?
Li3 P6 O26 Be4 -146.64(19) . . . . ?
Li3 P6 O26 Li8 79.25(15) . . . 4_454 ?
Li3 O16 Be7 O12 -20.9(2) . . . . ?
Li3 O16 Be7 O21 98.6(2) . . . 3_545 ?
Li3 O16 Be7 O31 -138.96(18) . . . 2_564 ?
Li3 O16 Be7 Li4 -15.9(4) . . . 2_564 ?
Li3 O16 Be7 Li7 139.41(19) . . . 2_564 ?
Li3 O16 Be7 Li8 -103.94(19) . . . 4_454 ?
Li3 O23 Be6 O10 167.94(17) 3_455 . . 1_565 ?
Li3 O23 Be6 O14 43.8(2) 3_455 . . 3_465 ?
Li3 O23 Be6 O25 -78.2(2) 3_455 . . . ?
Li3 O23 Be6 Li1 -120.68(18) 3_455 . . . ?
Li3 O23 Be6 Li5 27.0(4) 3_455 . . . ?
Li3 O23 Be6 Li6 154.61(16) 3_455 . . 1_565 ?
Li3 O28 Be5 O1 66.4(2) . . . 3_545 ?
Li3 O28 Be5 O8 -170.37(19) . . . . ?
Li3 O28 Be5 O17 -50.6(2) . . . . ?
Li3 O28 Be5 Li2 -16.3(3) . . . . ?
Li3 O28 Be5 Li4 104.78(18) . . . . ?
Li3 O28 Be5 Li5 -139.77(19) . . . 1_545 ?
Li4 P1 O8 Be5 49.98(18) . . . . ?
Li4 P1 O8 Li5 -160.06(19) . . . 1_545 ?
Li4 P1 O10 Be6 133.72(16) . . . 1_545 ?
Li4 P1 O10 Li6 -35.90(19) . . . . ?
Li4 P1 O15 Be2 164.6(3) . . . 2 ?
Li4 P1 O19 Be3 37.2(2) . . . . ?
Li4 P1 O19 Li1 166.10(16) . . . 1_545 ?
Li4 P2 O1 Be5 170.5(2) 3_455 . . 3_455 ?
Li4 P2 O9 Be4 24.4(2) 3_455 . . 2_565 ?
Li4 P2 O9 Li6 -143.4(2) 3_455 . . 1_565 ?
Li4 P2 O23 Be6 145.52(18) 3_455 . . . ?
Li4 P2 O23 Li3 -63.3(2) 3_455 . . 3_455 ?
Li4 P2 O30 Be1 -85.2(2) 3_455 . . . ?
Li4 P2 O30 Li2 48.51(18) 3_455 . . 3_455 ?
Li4 P4 O12 Be7 -139.7(2) 2_564 . . . ?
Li4 P4 O20 Be3 94.4(2) 2_564 . . 1_565 ?
Li4 P4 O20 Li3 -46.8(2) 2_564 . . . ?
Li4 P4 O22 Be2 33.24(19) 2_564 . . 1_565 ?
Li4 P4 O22 Li2 -125.2(2) 2_564 . . 1_565 ?
Li4 P4 O32 Be8 -148.37(17) 2_564 . . . ?
Li4 P4 O32 Li8 77.49(17) 2_564 . . 4_454 ?
Li4 P8 O6 Be4 -123.4(2) 4_454 . . . ?
Li4 P8 O13 Be1 -156.12(18) 4_454 . . . ?
Li4 P8 O13 Li5 57.6(2) 4_454 . . 1_545 ?
Li4 P8 O24 Be2 24.22(18) 4_454 . . 3_455 ?
Li4 P8 O24 Li7 -107.41(15) 4_454 . . 4_464 ?
Li4 P8 O27 Be8 26.4(3) 4_454 . . . ?
Li4 P8 O27 Li1 -180.0(2) 4_454 . . . ?
Li4 O6 Be4 O5 -62.00(19) 4_454 . . 1_545 ?
Li4 O6 Be4 O9 54.3(2) 4_454 . . 2_564 ?
Li4 O6 Be4 O26 176.07(18) 4_454 . . . ?
Li4 O6 Be4 Li5 -96.61(16) 4_454 . . 1_545 ?
Li4 O6 Be4 Li6 56.0(5) 4_454 . . 2_554 ?
Li4 O6 Be4 Li8 143.16(17) 4_454 . . 4_454 ?
Li4 O12 Be7 O16 176.33(18) 2_564 . . . ?
Li4 O12 Be7 O21 53.5(2) 2_564 . . 3_545 ?
Li4 O12 Be7 O31 -68.6(2) 2_564 . . 2_564 ?
Li4 O12 Be7 Li3 163.41(18) 2_564 . . . ?
Li4 O12 Be7 Li7 39.9(4) 2_564 . . 2_564 ?
Li4 O12 Be7 Li8 -108.60(18) 2_564 . . 4_454 ?
Li5 P5 O4 Be3 107.64(19) 3_535 . . . ?
Li5 P5 O4 Li2 -36.5(2) 3_535 . . . ?
Li5 P5 O14 Be6 126.5(3) 3_535 . . 3_535 ?
Li5 P5 O18 Be1 69.71(17) 3_535 . . 3_545 ?
Li5 P5 O18 Li8 -123.38(19) 3_535 . . . ?
Li5 P5 O29 Be8 50.7(3) 3_535 . . 4 ?
Li5 P5 O29 Li7 -148.17(19) 3_535 . . 1_545 ?
Li5 P7 O5 Be4 168.5(3) . . . 1_565 ?
Li5 P7 O7 Be8 151.38(17) . . . . ?
Li5 P7 O7 Li6 -69.75(17) . . . 2_564 ?
Li5 P7 O21 Be7 -28.5(2) . . . 3_455 ?
Li5 P7 O21 Li7 -165.59(17) . . . 4_464 ?
Li5 P7 O25 Be6 30.8(2) . . . . ?
Li5 P7 O25 Li1 -125.4(2) . . . . ?
Li5 O8 Be5 O1 168.56(17) 1_545 . . 3_545 ?
Li5 O8 Be5 O17 -74.79(19) 1_545 . . . ?
Li5 O8 Be5 O28 44.1(2) 1_545 . . . ?
Li5 O8 Be5 Li2 -120.74(17) 1_545 . . . ?
Li5 O8 Be5 Li3 27.5(5) 1_545 . . . ?
Li5 O8 Be5 Li4 154.54(15) 1_545 . . . ?
Li5 O13 Be1 O3 86.3(2) 1_545 . . . ?
Li5 O13 Be1 O18 -30.9(2) 1_545 . . 3_455 ?
Li5 O13 Be1 O30 -150.23(18) 1_545 . . . ?
Li5 O13 Be1 Li1 127.00(19) 1_545 . . . ?
Li5 O13 Be1 Li2 -119.70(17) 1_545 . . 3_455 ?
Li5 O13 Be1 Li8 -4.3(3) 1_545 . . 3_455 ?
Li6 P1 O8 Be5 146.51(18) . . . . ?
Li6 P1 O8 Li5 -63.54(19) . . . 1_545 ?
Li6 P1 O10 Be6 169.6(2) . . . 1_545 ?
Li6 P1 O15 Be2 23.5(2) . . . 2 ?
Li6 P1 O15 Li4 -141.08(19) . . . . ?
Li6 P1 O19 Be3 -82.9(2) . . . . ?
Li6 P1 O19 Li1 46.05(18) . . . 1_545 ?
Li6 P2 O1 Be5 133.54(16) 1_565 . . 3_455 ?
Li6 P2 O1 Li4 -36.95(18) 1_565 . . 3_455 ?
Li6 P2 O9 Be4 167.8(3) 1_565 . . 2_565 ?
Li6 P2 O23 Be6 49.40(18) 1_565 . . . ?
Li6 P2 O23 Li3 -159.4(2) 1_565 . . 3_455 ?
Li6 P2 O30 Be1 33.7(2) 1_565 . . . ?
Li6 P2 O30 Li2 167.47(16) 1_565 . . 3_455 ?
Li6 P6 O11 Be2 -122.8(2) 2_554 . . . ?
Li6 P6 O16 Be7 20.8(3) 2_554 . . . ?
Li6 P6 O16 Li3 173.76(19) 2_554 . . . ?
Li6 P6 O17 Be5 -130.7(2) 2_554 . . . ?
Li6 P6 O17 Li2 73.39(19) 2_554 . . . ?
Li6 P6 O26 Be4 25.80(19) 2_554 . . . ?
Li6 P6 O26 Li8 -108.31(16) 2_554 . . 4_454 ?
Li6 P7 O5 Be4 30.6(2) 2_564 . . 1_565 ?
Li6 P7 O5 Li5 -137.9(2) 2_564 . . . ?
Li6 P7 O7 Be8 -138.9(2) 2_564 . . . ?
Li6 P7 O21 Be7 -146.35(17) 2_564 . . 3_455 ?
Li6 P7 O21 Li7 76.56(17) 2_564 . . 4_464 ?
Li6 P7 O25 Be6 120.5(2) 2_564 . . . ?
Li6 P7 O25 Li1 -35.7(2) 2_564 . . . ?
Li6 O7 Be8 O27 174.72(18) 2_564 . . . ?
Li6 O7 Be8 O29 -69.5(2) 2_564 . . 4_454 ?
Li6 O7 Be8 O32 53.6(2) 2_564 . . . ?
Li6 O7 Be8 Li1 153.1(2) 2_564 . . . ?
Li6 O7 Be8 Li7 -109.43(17) 2_564 . . 4_464 ?
Li6 O7 Be8 Li8 42.1(4) 2_564 . . 4_454 ?
Li6 O11 Be2 O15 55.0(2) 2_554 . . 2_554 ?
Li6 O11 Be2 O22 -62.9(2) 2_554 . . 1_545 ?
Li6 O11 Be2 O24 177.50(18) 2_554 . . 3_545 ?
Li6 O11 Be2 Li2 -105.97(17) 2_554 . . . ?
Li6 O11 Be2 Li4 52.6(4) 2_554 . . 2_554 ?
Li6 O11 Be2 Li7 143.72(17) 2_554 . . 2_564 ?
Li7 P3 O2 Be3 -172.3(2) . . . 1_565 ?
Li7 P3 O3 Be1 -145.10(18) . . . . ?
Li7 P3 O3 Li1 70.29(19) . . . . ?
Li7 P3 O28 Be5 82.1(2) . . . . ?
Li7 P3 O28 Li3 -43.12(17) . . . . ?
Li7 P3 O31 Be7 -20.6(2) . . . 2_565 ?
Li7 P3 O31 Li8 140.77(19) . . . 3_455 ?
Li7 P5 O4 Be3 -50.66(18) 1_545 . . . ?
Li7 P5 O4 Li2 165.2(2) 1_545 . . . ?
Li7 P5 O14 Be6 -41.4(2) 1_545 . . 3_535 ?
Li7 P5 O14 Li5 -167.94(17) 1_545 . . 3_535 ?
Li7 P5 O18 Be1 -130.66(16) 1_545 . . 3_545 ?
Li7 P5 O18 Li5 159.63(14) 1_545 . . 3_535 ?
Li7 P5 O18 Li8 36.3(2) 1_545 . . . ?
Li7 P5 O29 Be8 -161.1(3) 1_545 . . 4 ?
Li7 P7 O5 Be4 -45.8(3) 4_464 . . 1_565 ?
Li7 P7 O5 Li5 145.7(2) 4_464 . . . ?
Li7 P7 O7 Be8 -29.16(17) 4_464 . . . ?
Li7 P7 O7 Li6 109.71(17) 4_464 . . 2_564 ?
Li7 P7 O21 Be7 137.1(2) 4_464 . . 3_455 ?
Li7 P7 O25 Be6 -129.3(2) 4_464 . . . ?
Li7 P7 O25 Li1 74.57(17) 4_464 . . . ?
Li7 P8 O6 Be4 152.53(17) 4_464 . . . ?
Li7 P8 O6 Li4 -84.10(17) 4_464 . . 4_454 ?
Li7 P8 O13 Be1 -44.3(3) 4_464 . . . ?
Li7 P8 O13 Li5 169.4(2) 4_464 . . 1_545 ?
Li7 P8 O24 Be2 131.6(2) 4_464 . . 3_455 ?
Li7 P8 O27 Be8 -42.38(19) 4_464 . . . ?
Li7 P8 O27 Li1 111.2(2) 4_464 . . . ?
Li8 P3 O2 Be3 -134.99(17) 3_455 . . 1_565 ?
Li8 P3 O2 Li7 37.3(2) 3_455 . . . ?
Li8 P3 O3 Be1 -49.41(18) 3_455 . . . ?
Li8 P3 O3 Li1 166.0(2) 3_455 . . . ?
Li8 P3 O28 Be5 -38.3(2) 3_455 . . . ?
Li8 P3 O28 Li3 -163.50(17) 3_455 . . . ?
Li8 P3 O31 Be7 -161.4(3) 3_455 . . 2_565 ?
Li8 P4 O12 Be7 -29.86(17) 4_454 . . . ?
Li8 P4 O12 Li4 109.85(17) 4_454 . . 2_564 ?
Li8 P4 O20 Be3 -156.74(19) 4_454 . . 1_565 ?
Li8 P4 O20 Li3 62.00(19) 4_454 . . . ?
Li8 P4 O22 Be2 -41.6(3) 4_454 . . 1_565 ?
Li8 P4 O22 Li2 160.0(3) 4_454 . . 1_565 ?
Li8 P4 O32 Be8 134.1(3) 4_454 . . . ?
Li8 P5 O4 Be3 -145.92(18) . . . . ?
Li8 P5 O4 Li2 70.0(2) . . . . ?
Li8 P5 O14 Be6 79.3(2) . . . 3_535 ?
Li8 P5 O14 Li5 -47.26(18) . . . 3_535 ?
Li8 P5 O18 Be1 -166.9(2) . . . 3_545 ?
Li8 P5 O18 Li5 123.38(19) . . . 3_535 ?
Li8 P5 O29 Be8 -21.4(2) . . . 4 ?
Li8 P5 O29 Li7 139.70(19) . . . 1_545 ?
Li8 P6 O11 Be2 152.02(17) 4_454 . . . ?
Li8 P6 O11 Li6 -85.14(17) 4_454 . . 2_554 ?
Li8 P6 O16 Be7 -45.51(19) 4_454 . . . ?
Li8 P6 O16 Li3 107.45(17) 4_454 . . . ?
Li8 P6 O17 Be5 -15.5(3) 4_454 . . . ?
Li8 P6 O17 Li2 -171.4(2) 4_454 . . . ?
Li8 P6 O26 Be4 134.1(2) 4_454 . . . ?
Li8 O26 Be4 O5 -172.46(17) 4_454 . . 1_545 ?
Li8 O26 Be4 O6 -54.7(2) 4_454 . . . ?
Li8 O26 Be4 O9 68.0(2) 4_454 . . 2_564 ?
Li8 O26 Be4 Li4 -48.0(4) 4_454 . . 4_454 ?
Li8 O26 Be4 Li5 -142.52(15) 4_454 . . 1_545 ?
Li8 O26 Be4 Li6 105.17(17) 4_454 . . 2_554 ?
Li8 O32 Be8 O7 -172.56(18) 4_454 . . . ?
Li8 O32 Be8 O27 67.3(2) 4_454 . . . ?
Li8 O32 Be8 O29 -51.4(2) 4_454 . . 4_454 ?
Li8 O32 Be8 Li1 113.84(17) 4_454 . . . ?
Li8 O32 Be8 Li6 -139.85(17) 4_454 . . 2_564 ?
Li8 O32 Be8 Li7 -42.8(5) 4_454 . . 4_464 ?

_olex2_submission_special_instructions 'No special instructions were received'
